Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- solution for Materials Science and ... by shayangreen 120744 views
- [Solutions manual] engineering ma... by sametron90 148868 views
- Donald r . solution by abfisho 25965 views
- Materiales the science and engine... by Meylis Hydyrow 14162 views
- Materials science and engineering a... by Mukesh Achla 9223 views
- Callister fundamentals of materia... by p09ch807 10678 views

58,510 views

Published on

material science

No Downloads

Total views

58,510

On SlideShare

0

From Embeds

0

Number of Embeds

32

Shares

0

Downloads

2,235

Comments

3

Likes

41

No embeds

No notes for slide

- 1. Complete Solutions to Selected Problems to accompany MATERIALS SCIENCE AND ENGINEERING AN INTRODUCTION Sixth Edition William D. Callister, Jr. The University of Utah John Wiley & Sons, Inc.
- 2. Copyright 2003 John Wiley & Sons, Inc. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning or otherwise, except as permitted under Sections 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate per-copy fee to the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA 01923, (508)750-8400, fax (508)7504470. Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 605 Third Avenue, New York, NY 10158-0012, (212) 850-6011, fax (212) 850-6008, E-Mail: PERMREQ@WILEY.COM. To order books or for customer service please call 1(800)225-5945.
- 3. SOLUTIONS TO PROBLEMS PREFACE This section of instructor's resource materials contains solutions and answers to all problems and questions that appear in the textbook. My penmanship leaves something to be desired; therefore, I generated these solutions/answers using computer software so that the resulting product would be "readable." Furthermore, I endeavored to provide complete and detailed solutions in order that: (1) the instructor, without having to take time to solve a problem, will understand what principles/skills are to be learned by its solution; and (2) to facilitate student understanding/learning when the solution is posted. I would recommend that the course instructor consult these solutions/answers before assigning problems and questions. In doing so, he or she ensures that the students will be drilled in the intended principles and concepts. In addition, the instructor may provide appropriate hints for some of the more difficult problems. With regard to symbols, in the text material I elected to boldface those symbols that are italicized in the textbook. Furthermore, I also endeavored to be consistent relative to symbol style. However, in several instances, symbols that appear in the textbook were not available, and it was necessary to make appropriate substitutions. These include the following: the letter a (unit cell edge length, crack length) is used in place of the cursive a. And Roman E and F replace script E (electric field in Chapter 18) and script F (Faraday's constant in Chapter 17), respectively. I have exercised extreme care in designing these problems/questions, and then in solving them. However, no matter how careful one is with the preparation of a work such as this, errors will always remain in the final product. Therefore, corrections, suggestions, and comments from instructors who use the textbook (as well as their teaching assistants) pertaining to homework problems/solutions are welcomed. These may be sent to me in care of the publisher. 1
- 4. CHAPTER 2 ATOMIC STRUCTURE AND INTERATOMIC BONDING PROBLEM SOLUTIONS 2.1 (a) When two or more atoms of an element have different atomic masses, each is termed an isotope. (b) The atomic weights of the elements ordinarily are not integers because: (1) the atomic masses of the atoms generally are not integers (except for 12 C), and (2) the atomic weight is taken as the weighted average of the atomic masses of an atom's naturally occurring isotopes. 2.2 Atomic mass is the mass of an individual atom, whereas atomic weight is the average (weighted) of the atomic masses of an atom's naturally occurring isotopes. 2.3 (a) In order to determine the number of grams in one amu of material, appropriate manipulation of the amu/atom, g/mol, and atom/mol relationships is all that is necessary, as ⎛ ⎞ ⎛ 1 g / mol ⎞ 1 mol # g/amu = ⎜ ⎜ ⎟ 23 atoms ⎟ ⎝ 1 amu / atom ⎠ ⎝ 6.023 x 10 ⎠ = 1.66 x 10-24 g/amu (b) Since there are 453.6 g/lbm, ( )( 23 1 lb - mol = 453.6 g/lbm 6.023 x 10 ) atoms/g - mol = 2.73 x 1026 atoms/lb-mol 2.4 (a) Two important quantum-mechanical concepts associated with the Bohr model of the atom are that electrons are particles moving in discrete orbitals, and electron energy is quantized into shells. (b) Two important refinements resulting from the wave-mechanical atomic model are that electron position is described in terms of a probability distribution, and electron energy is quantized into both shells and subshells--each electron is characterized by four quantum numbers. 2.5 The n quantum number designates the electron shell. 2
- 5. The l quantum number designates the electron subshell. The m quantum number designates the number of electron states in each electron subshell. l The m quantum number designates the spin moment on each electron. s 2.6 For the L state, n = 2, and eight electron states are possible. Possible l values are 0 and 1, while 1 possible ml values are 0 and ±1. Therefore, for the s states, the quantum numbers are 200 ( ) and 2 1 1 1 1 2 1 2 2 2 200 (− ) . For the p states, the quantum numbers are 210 ( ) , 210 (− ) , 211 ( ) , 211 (− ) , 2 1 1 2 2 21(-1 )( ) , and 21(-1 )(− ) . For the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2; 1 possible ml values are 0, ±1, and ±2; and possible ms values are ± . Therefore, for the s states, 2 1 1 1 1 2 1 2 1 2 1 2 1 2 2 the quantum numbers are 300 ( ) , 300 (− ) , for the p states they are 310 ( ) , 310 (− ) , 311 ( ) , 2 1 1 1 2 1 2 1 2 1 1 1 1 1 2 2 2 2 2 2 2 311 (− ) , 31(-1 )( ) , and 31(-1 )(− ) ; for the d states they are 320 ( ) , 320 (− ) , 321 ( ) , 2 321 (− ) , 32(-1 )( ) , 32(-1 )(− ) , 322 ( ) , 322 (− ) , 32(-2) ( ) , and 32(-2) (− ) . 2.7 The electron configurations of the ions are determined using Table 2.2. 2 2 6 2 6 6 - 1s 2s 2p 3s 3p 3d 3+ 2 2 6 2 6 5 Fe - 1s 2s 2p 3s 3p 3d + 2 2 6 2 6 10 Cu - 1s 2s 2p 3s 3p 3d 2+ 2 2 6 2 6 10 2 6 10 2 6 Ba - 1s 2s 2p 3s 3p 3d 4s 4p 4d 5s 5p 2 2 6 2 6 10 2 6 Br - 1s 2s 2p 3s 3p 3d 4s 4p 22 2 6 2 6 S - 1s 2s 2p 3s 3p Fe 2.8 2+ + The Na ion is just a sodium atom that has lost one electron; therefore, it has an electron configuration the same as neon (Figure 2.6). The Cl ion is a chlorine atom that has acquired one extra electron; therefore, it has an electron configuration the same as argon. 2.9 Each of the elements in Group IIA has two s electrons. 2 2 6 2 6 7 2 2.10 (a) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of an incomplete d subshell. 3
- 6. 2 2 6 2 6 (b) The 1s 2s 2p 3s 3p electron configuration is that of an inert gas because of filled 3s and 3p subshells. 2 2 5 (c) The 1s 2s 2p electron configuration is that of a halogen because it is one electron deficient from having a filled L shell. 2 2 6 2 (d) The 1s 2s 2p 3s electron configuration is that of an alkaline earth metal because of two s electrons. 2 2 6 2 6 2 2 (e) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of an incomplete d subshell. 2 2 6 2 6 1 (f) The 1s 2s 2p 3s 3p 4s electron configuration is that of an alkali metal because of a single s electron. 2.11 (a) The 4f subshell is being filled for the rare earth series of elements. (b) The 5f subshell is being filled for the actinide series of elements. 2.12 The attractive force between two ions FA is just the derivative with respect to the interatomic separation of the attractive energy expression, Equation (2.8), which is just FA = dE A dr ⎛ A⎞ d⎜− ⎟ ⎝ r⎠ A = = 2 dr r The constant A in this expression is defined in footnote 3. Since the valences of the Ca2+ and O2ions (Z1 and Z2) are both 2, then FA = (Z1e )(Z2e) 4πεor 2 ( −19 (2)(2 ) 1.6 x 10 = ( (4)(π) 8.85 x 10 −12 ) C )( 2 F / m) 1.25 x 10 = 5.89 x 10-10 N 2.13 (a) Differentiation of Equation (2.11) yields dEN dr = A − r(1 + 1) 4 nB r(n + 1) = 0 −9 ) m 2
- 7. (b) Now, solving for r (= r ) o A ro 2 nB = ro(n + 1) or ⎛ A⎞ ro = ⎜ ⎟ ⎝ nB ⎠ 1/(1 - n) (c) Substitution for ro into Equation (2.11) and solving for E (= Eo) Eo = − = − A B + r ron o A ⎛ A⎞ ⎜ ⎟ ⎝ nB ⎠ 1/(1 - n) + B ⎛ A⎞ ⎜ ⎟ ⎝ nB ⎠ n/(1 - n) 2.14 (a) Curves of E , E , and E are shown on the plot below. A R N 5
- 8. (b) From this plot r = 0.24 nm o E = -5.3 eV o (c) From Equation (2.11) for E N A = 1.436 -6 B = 7.32 x 10 n=8 Thus, ⎛ A⎞ ro = ⎜ ⎟ ⎝ nB ⎠ ⎡ 1.436 ⎢ = ⎢ -6 ⎢(8) 7.32 x 10 ⎣ ( 1/(1 - n) 1/(1 - 8) ⎤ ⎥ ⎥ ⎥ ⎦ = 0.236 nm ) and Eo = − 1.436 ⎡ ⎤ 1.436 ⎢ ⎥ ⎢ (8) ⎛ 7.32 x 10−6 ⎞ ⎥ ⎠⎦ ⎣ ⎝ 1/(1 − 8) + 7.32 x 10 −6 ⎡ ⎤ 1.436 ⎢ ⎥ ⎢ (8) ⎛ 7.32 x 10 −6 ⎞ ⎥ ⎠⎦ ⎣ ⎝ 8 /(1 − 8) = - 5.32 eV 2.15 This problem gives us, for a hypothetical X+-Y- ion pair, values for ro (0.35 nm), Eo (-6.13 eV), and n (10), and asks that we determine explicit expressions for attractive and repulsive energies of Equations 2.8 and 2.9. In essence, it is necessary to compute the values of A and B in these equations. Expressions for ro and Eo in terms of n, A, and B were determined in Problem 2.13, which are as follows: ⎛ A⎞ ro = ⎜ ⎟ ⎝ nB ⎠ 6 1/(1 - n)
- 9. Eo = − A ⎛ A⎞ ⎜ ⎟ ⎝ nB ⎠ + 1/(1 - n) B ⎛ A⎞ ⎜ ⎟ ⎝ nB ⎠ n/(1 - n) Thus, we have two simultaneous equations with two unknowns (viz. A and B). Upon substitution of values for ro and Eo in terms of n, these equations take the forms ⎛ A ⎞ 1/(1 - 10) 0.35 nm = ⎜ ⎟ ⎝ 10B ⎠ − 6.13 eV = − A ⎛ A ⎞ ⎜ ⎟ ⎝ 10B ⎠ 1/(1 − 10) + B ⎛ A ⎞ ⎜ ⎟ ⎝ 10B ⎠ 10 /(1 − 10) Simultaneous solution of these two equations leads to A = 2.38 and B = 1.88 x 10-5. Thus, Equations (2.8) and (2.9) become 2.38 r EA = − ER = 1.88 x 10 −5 r10 Of course these expressions are valid for r and E in units of nanometers and electron volts, respectively. 2.16 (a) Differentiating Equation (2.12) with respect to r yields −r / ρ dE C De = − 2 dr ρ r At r = ro, dE/dr = 0, and C ro 2 = De − (ro /ρ) ρ Solving for C and substitution into Equation (2.12) yields an expression for Eo as 7 (2.12b)
- 10. Eo = De ro ⎞ ⎟ ⎜1 − ρ⎠ ⎝ − (ro/ρ) ⎛ (b) Now solving for D from Equation (2.12b) above yields D = Cρe (ro/ρ) ro2 Substitution of this expression for D into Equation (2.12) yields an expression for Eo as Eo = ⎞ C⎛ ρ ⎜ − 1⎟ ⎟ r ⎜r ⎠ o⎝ o 2.17 (a) The main differences between the various forms of primary bonding are: Ionic--there is electrostatic attraction between oppositely charged ions. Covalent--there is electron sharing between two adjacent atoms such that each atom assumes a stable electron configuration. Metallic--the positively charged ion cores are shielded from one another, and also "glued" together by the sea of valence electrons. (b) The Pauli exclusion principle states that each electron state can hold no more than two electrons, which must have opposite spins. 2.18 Covalently bonded materials are less dense than metallic or ionically bonded ones because covalent bonds are directional in nature whereas metallic and ionic are not; when bonds are directional, the atoms cannot pack together in as dense a manner, yielding a lower mass density. 2.19 The percent ionic character is a function of the electron negativities of the ions XA and XB according to Equation (2.10). The electronegativities of the elements are found in Figure 2.7. For MgO, XMg = 1.2 and XO = 3.5, and therefore, 2⎤ ⎡ %IC = ⎢1 − e (− 0.25) (3.5 − 1.2) ⎥ x 100 = 73.4% ⎦ ⎣ For GaP, XGa = 1.6 and XP = 2.1, and therefore, 8
- 11. 2⎤ ⎡ %IC = ⎢1 − e (− 0.25) (2.1−1.6) ⎥ x 100 = 6.1% ⎦ ⎣ For CsF, XCs = 0.7 and XF = 4.0, and therefore, 2⎤ ⎡ %IC = ⎢1 − e (− 0.25) (4.0 − 0.7) ⎥ x 100 = 93.4% ⎦ ⎣ For CdS, XCd = 1.7 and XS = 2.5, and therefore, 2⎤ ⎡ %IC = ⎢1 − e (− 0.25) (2.5 − 1.7 ) ⎥ x 100 = 14.8% ⎦ ⎣ For FeO, XFe = 1.8 and XO = 3.5, and therefore, 2⎤ ⎡ %IC = ⎢1 − e (− 0.25) (3.5 − 1.8) ⎥ x 100 = 51.4% ⎦ ⎣ 2.20 Below is plotted the bonding energy versus melting temperature for these four metals. From this plot, the bonding energy for copper (melting temperature of 1084°C) should be approximately 3.6 eV. The experimental value is 3.5 eV. 9
- 12. 2 2 2.21 For silicon, having the valence electron structure 3s 3p , N' = 4; thus, there are 8 - N' = 4 covalent bonds per atom. 2 5 For bromine, having the valence electron structure 4s 4p , N' = 7; thus, there is 8 - N' = 1 covalent bond per atom. 2 3 For nitrogen, having the valence electron structure 2s 2p , N' = 5; thus, there are 8 - N' = 3 covalent bonds per atom. 2 4 For sulfur, having the valence electron structure 3s 3p , N' = 6; thus, there are 8 - N' = 2 covalent bonds per atom. 2.22 For brass, the bonding is metallic since it is a metal alloy. For rubber, the bonding is covalent with some van der Waals. (Rubber is composed primarily of carbon and hydrogen atoms.) For BaS, the bonding is predominantly ionic (but with some covalent character) on the basis of the relative positions of Ba and S in the periodic table. For solid xenon, the bonding is van der Waals since xenon is an inert gas. For bronze, the bonding is metallic since it is a metal alloy (composed of copper and tin). For nylon, the bonding is covalent with perhaps some van der Waals. (Nylon is composed primarily of carbon and hydrogen.) For AlP the bonding is predominantly covalent (but with some ionic character) on the basis of the relative positions of Al and P in the periodic table. 2.23 The intermolecular bonding for HF is hydrogen, whereas for HCl, the intermolecular bonding is van der Waals. Since the hydrogen bond is stronger than van der Waals, HF will have a higher melting temperature. 2.24 The geometry of the H O molecules, which are hydrogen bonded to one another, is more restricted 2 in the solid phase than for the liquid. This results in a more open molecular structure in the solid, and a less dense solid phase. 10
- 13. CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS 3.1 Atomic structure relates to the number of protons and neutrons in the nucleus of an atom, as well as the number and probability distributions of the constituent electrons. On the other hand, crystal structure pertains to the arrangement of atoms in the crystalline solid material. 3.2 A crystal structure is described by both the geometry of, and atomic arrangements within, the unit cell, whereas a crystal system is described only in terms of the unit cell geometry. For example, face-centered cubic and body-centered cubic are crystal structures that belong to the cubic crystal system. 3.3 For this problem, we are asked to calculate the volume of a unit cell of aluminum. Aluminum has an FCC crystal structure (Table 3.1). The FCC unit cell volume may be computed from Equation (3.4) as VC = 16R 3 ( -9 2 = (16) 0.143 x 10 ) m 3 2 = 6.62 x 10 3.4 This problem calls for a demonstration of the relationship a = 4R unit cell shown below Using the triangle NOP 11 -29 3 m 3 for BCC. Consider the BCC
- 14. (NP)2 = a 2 + a 2 = 2a 2 And then for triangle NPQ, (NQ)2 = (QP )2 + (NP)2 But NQ = 4R, R being the atomic radius. Also, QP = a. Therefore, (4R)2 = a 2 + 2a2 , or a = 4R 3 3.5 We are asked to show that the ideal c/a ratio for HCP is 1.633. A sketch of one-third of an HCP unit cell is shown below. Consider the tetrahedron labeled as JKLM, which is reconstructed as 12
- 15. The atom at point M is midway between the top and bottom faces of the unit cell--that is MH = c/2. And, since atoms at points J, K, and M, all touch one another, JM = JK = 2R = a where R is the atomic radius. Furthermore, from triangle JHM, (JM) 2 = (JH)2 + (MH)2, or a 2 2 = (JH ) ⎛ c⎞ + ⎜ ⎟ ⎝ 2⎠ 2 Now, we can determine the JH length by consideration of triangle JKL, which is an equilateral triangle, cos 30° = a/ 2 = JH JH = 3 , and 2 a 3 Substituting this value for JH in the above expression yields 2 2 ⎛ a ⎞ a2 c2 ⎛ c⎞ a2 = ⎜ + ⎜ ⎟ = + ⎟ ⎝ 2⎠ 3 4 ⎝ 3⎠ and, solving for c/a 13
- 16. c = a 8 = 1.633 3 3.6 We are asked to show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = VS VC Since there are two spheres associated with each unit cell for BCC 3 ⎛ 4πR 3 ⎞ 8πR VS = 2(sphere volume) = 2 ⎜ ⎟= ⎜ 3 ⎟ 3 ⎝ ⎠ 3 Also, the unit cell has cubic symmetry, that is V = a . But a depends on R according to Equation C (3.3), and ⎛ 4R ⎞ VC = ⎜ ⎟ ⎝ 3⎠ 3 = 64R 3 3 3 Thus, APF = 8πR 3 / 3 64R 3 / 3 3 = 0.68 3.7 This problem calls for a demonstration that the APF for HCP is 0.74. Again, the APF is just the total sphere-unit cell volume ratio. For HCP, there are the equivalent of six spheres per unit cell, and thus ⎛ 4π R3 ⎞ 3 VS = 6 ⎜ ⎜ 3 ⎟ = 8πR ⎟ ⎝ ⎠ Now, the unit cell volume is just the product of the base area times the cell height, c. This base area is just three times the area of the parallelepiped ACDE shown below. 14
- 17. The area of ACDE is just the length of CD times the height BC . But CD is just a or 2R, and BC = 2R cos (30°) = 2R 3 2 Thus, the base area is just ⎛ 2R 3 ⎞ 2 AREA = (3)(CD )(BC) = (3)(2 R) ⎜ ⎟ = 6R 3 2 ⎠ ⎝ and since c = 1.633a = 2R(1.633) ( 2 2 VC = (AREA)(c) = 6R c 3 = 6 R ) 3 (2)(1.633)R = 12 3 (1.633 )R 3 Thus, APF = VS VC 3 = 8π R 12 3 (1.633 )R 3 = 0.74 3.8 This problem calls for a computation of the density of iron. According to Equation (3.5) ρ = nAFe VC NA For BCC, n = 2 atoms/unit cell, and 15
- 18. ⎛ 4R ⎞ VC = ⎜ ⎟ ⎝ 3⎠ 3 Thus, ρ = (2 atoms/unit cell)(55.9 g/mol) 3 ⎫ ⎧⎡ 3 ⎤ ⎪ ⎪ -7 23 ⎨⎢(4 ) 0.124 x 10 cm / 3 ⎥ /(unit cell)⎬ 6.023 x 10 atoms/mol ⎪ ⎪⎣ ⎦ ⎭ ⎩ ( ) ( ) = 7.90 g/cm3 3 The value given inside the front cover is 7.87 g/cm . 3.9 We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal structure. For FCC, n = 4 atoms/unit cell, and V = 16R C 3 ρ = 2 [Equation (3.4)]. Now, nAIr V N C A And solving for R from the above two expressions yields ⎞ ⎛ nA Ir ⎟ R = ⎜ ⎜ 16ρN 2 ⎟ ⎠ ⎝ A ⎡ ⎢ = ⎢ ⎢ ⎣ ( 1/3 (4 atoms/unit cell)(192.2 g/mol) 2 )16) 22.4 g/cm3 6.023 x 10 23 atoms/mol ( ( ) ( ⎤ ⎥ ⎥ ⎥ ⎦ 1/3 ) = 1.36 x 10-8 cm = 0.136 nm 3.10 This problem asks for us to calculate the radius of a vanadium atom. For BCC, n = 2 atoms/unit cell, and ⎛ 4R ⎞ VC = ⎜ ⎟ ⎝ 3⎠ 16 3 = 64R 3 3 3
- 19. Since, ρ = nAV V N C A and solving for R ⎛ 3 n 3A ⎞ V⎟ R = ⎜ ⎜ 64ρN ⎟ A ⎠ ⎝ 1/3 ⎡ 3 3 (2 atoms/unit cell)(50.9 g/mol) ⎢ = ⎢ 3 23 atoms/mol ⎢ (64) 5.96 g/cm 6.023 x 10 ⎣ ( ) ( )( ⎤ ⎥ ⎥ ⎥ ⎦ 1/3 ) = 1.32 x 10-8 cm = 0.132 nm 3.11 For the simple cubic crystal structure, the value of n in Equation (3.5) is unity since there is only a single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R. Therefore, employment of Equation (3.5) yields ρ = nA V N = C A = nA (2R )3N A (1 atom/unit cell)(74.5 g/mol) 3 ⎫ ⎧ ⎪ ⎪⎡ 23 -8 ⎤ ⎨⎢(2) 1.45 x 10 cm ⎥ /(unit cell)⎬ 6.023 x 10 atoms/mol ⎦ ⎪ ⎪⎣ ⎭ ⎩ ( ) ( 5.07 g/cm3 3.12. (a) The volume of the Ti unit cell may be computed using Equation (3.5) as VC = nATi ρN Now, for HCP, n = 6 atoms/unit cell, and for Ti, A 17 A Ti = 47.9 g/mol. Thus, )
- 20. VC = (6 atoms/unit cell)(47.9 g/mol) 23 3 4.51 g/cm 6.023 x 10 atoms/mol ( ) ( ) = 1.058 x 10-22 cm3/unit cell = 1.058 x 10-28 m3/unit cell (b) From the solution to Problem 3.7, since a = 2R, then, for HCP VC = 3 3 a 2c 2 but, since c = 1.58a VC = 3 3 (1.58)a 3 -22 3 = 1.058 x 10 cm /unit cell 2 Now, solving for a ( ⎡ 2 1.058 x 10-22 cm3 ⎢( ) a = ⎢ (3 ) 3 (1.58) ⎢ ⎣ ( ) )⎤⎥ 1/3 ⎥ ⎥ ⎦ = 2.96 x 10-8 cm = 0.296 nm And finally c = 1.58a = (1.58)(0.296 nm) = 0.468 nm 3.13 This problem asks that we calculate the theoretical densities of Al, Ni, Mg, and W. ( Since Al has an FCC crystal structure, n = 4, and VC = 2R 2 )3 . Also, R = 0.143 nm (1.43 x 10-8 cm) and AAl = 26.98 g/mol. Employment of Equation (3.5) yields ρ = (4 atoms/unit cell)(26.98 g/mol) 3 ⎧ ⎫ -8 23 atoms/mol ⎨ (2)(1.43 x 10 cm) 2 /(unit cell) ⎬ 6.023 x 10 ⎩ ⎭ [ ( )] ( = 2.71 g/cm3 The value given in the table inside the front cover is 2.71 g/cm3. 18 )
- 21. Nickel also has an FCC crystal structure and therefore ρ = (4 atoms/unit cell)(58.69 g/mol) 3 ⎧ ⎫ -8 23 atoms/mol ⎨ (2)(1.25 x 10 cm) 2 /(unit cell )⎬ 6.023 x 10 ⎩ ⎭ [ ( )] ( ) = 8.82 g/cm3 The value given in the table is 8.90 g/cm3. Magnesium has an HCP crystal structure, and from Problem 3.7, 3 3 a 2c 2 VC = and, since c = 1.624a and a = 2R = 2(1.60 x 10-8 cm) = 3.20 x 10-8 cm ( ) 3 3 (1.624) 3.20 x 10-8 cm VC = 3 2 −22 = 1.38 x 10 3 cm /unit cell Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is ρ = nAMg V N C A = (6 atoms/unit cell)(24.31 g/mol) -22 3 23 1.38 x 10 cm /unit cell 6.023 x 10 atoms/mol ( ) ( ) = 1.75 g/cm3 The value given in the table is 1.74 g/cm3. Tungsten has a BCC crystal structure for which n = 2 and a = and R = 0.137 nm. Therefore, employment of Equation (3.5) leads to 19 4R ; also AW = 183.85 g/mol 3
- 22. ρ = (2 atoms/unit cell)(183.85 g/mol) ( ) 3 ⎫ ⎧⎡ -8 ⎤ ⎪ ⎪⎢(4 ) 1.37 x 10 cm ⎥ ⎪ ⎪ /(unit cell)⎬ 6.023 x 1023 atoms/mol ⎨⎢ ⎥ 3 ⎪ ⎪⎢ ⎥ ⎦ ⎪ ⎪ ⎭ ⎩⎣ ( ) = 19.3 g/cm3 The value given in the table is 19.3 g/cm3. 3.14 In order to determine whether Nb has an FCC or BCC crystal structure, we need to compute its density for each of the crystal structures. For FCC, n = 4, and a = 2 R 2 . Also, from Figure 2.6, its atomic weight is 92.91 g/mol. Thus, for FCC ρ = nA Nb 3 2R 2 N A ( ) (4 atoms/unit cell)(92.91 g/mol) 3 ⎧⎡ ⎫ -8 23 2 ⎤ /(unitcell)⎬ 6.023 x 10 atoms / mol ⎨ (2) 1.43 x 10 cm ⎣ ⎦ ⎩ ⎭ = ( )( ) ( ) = 9.33 g/cm3 For BCC, n = 2, and a = = 4R , thus 3 (2 atoms/unit cell)(92.91 g/mol) 3 ⎧ ⎫ -8 ⎡ ⎪ (4) 1.43 x 10 cm ⎤ ⎪ ⎢ 23 ⎥ /(unitcell) ⎨ ⎬ 6.023 x 10 atoms/ mol ⎢ ⎥ 3 ⎪⎢ ⎪ ⎥ ⎦ ⎪⎣ ⎪ ⎩ ⎭ ( ) ( ) = 8.57 g/cm3 which is the value provided in the problem. Therefore, Nb has a BCC crystal structure. 3.15 For each of these three alloys we need to, by trial and error, calculate the density using Equation (3.5), and compare it to the value cited in the problem. For SC, BCC, and FCC crystal structures, 20
- 23. the respective values of n are 1, 2, and 4, whereas the expressions for a (since VC = a3) are 2R, 2 R 2 , and 4R / 3 . For alloy A, let us calculate ρ assuming a BCC crystal structure. ρ = nAA V N C A = (2 atoms/unit cell)(43.1 g/mol) 3 ⎫ ⎧ -8 ⎡ ⎤ ⎪ ⎪⎢ (4) 1.22 x 10 cm ⎥ ⎪ ⎪ /(unit cell)⎬ 6.023 x 1023 atoms/mol ⎨⎢ ⎥ 3 ⎪ ⎪⎢ ⎥ ⎦ ⎪ ⎪⎣ ⎭ ⎩ ( ) ( ) = 6.40 g/cm3 Therefore, its crystal structure is BCC. For alloy B, let us calculate ρ assuming a simple cubic crystal structure. ρ = (1 atom/unit cell)(184.4 g/mol) 3 ⎧ ⎫ ⎪⎡ ⎪ ⎤ -8 23 ⎨⎢(2 ) 1.46 x 10 cm ⎥ /(unit cell)⎬ 6.023 x 10 atoms/mol ⎦ ⎪⎣ ⎪ ⎩ ⎭ ( ) ( ) = 12.3 g/cm3 Therefore, its crystal structure is simple cubic. For alloy C, let us calculate ρ assuming a BCC crystal structure. ρ = (2 atoms/unit cell)(91.6 g/mol) 3 ⎫ ⎧ -8 ⎡ ⎤ ⎪ ⎪⎢(4) 1.37 x 10 cm ⎥ ⎪ ⎪ /(unit cell)⎬ 6.023 x 1023 atoms/mol ⎨⎢ ⎥ 3 ⎪ ⎪⎢ ⎥ ⎦ ⎪ ⎪⎣ ⎭ ⎩ ( ) ( = 9.60 g/cm3 Therefore, its crystal structure is BCC. 21 )
- 24. 3.16 In order to determine the APF for U, we need to compute both the unit cell volume (VC) which is just the product of the three unit cell parameters, as well as the total sphere volume (VS) which is just the product of the volume of a single sphere and the number of spheres in the unit cell (n). The value of n may be calculated from Equation (3.5) as ρVC NA n = AU ( ) ( (19.05)(2.86)(5.87)(4.95) x10 -24 6.023 x 1023 = 283.03 = 4.01 atoms/unit cell Therefore ⎞ ⎛4 (4) ⎜ π R3 ⎟ ⎠ ⎝3 APF = = VC (a)(b)(c) VS ⎡4 3⎤ (4)⎢ (π)(0.1385) ⎥ ⎣3 ⎦ = (0.286)(0.587)(0.495) = 0.536 3.17 (a) From the definition of the APF APF = VS VC = ⎞ ⎛4 n ⎜ πR 3 ⎟ ⎠ ⎝3 a 2c we may solve for the number of atoms per unit cell, n, as 2 n = (APF)a c 4 πR 3 3 22 )
- 25. ( (0.693)(4.59)2(4.95) 10 -24 cm3 = ( ) 4 π 1.625 x 10-8 cm 3 ) 3 = 4.0 atoms/unit cell (b) In order to compute the density, we just employ Equation (3.5) as nAIn ρ = a2 c N A = (4 atoms/unit cell)(114.82 g/mol) 2 ⎤ ⎡ 23 -8 -8 atoms/mol ⎢ 4.59 x 10 cm 4.95 x 10 cm /unit cell ⎥ 6.023 x 10 ⎦ ⎣ ( )( ( ) ) = 7.31 g/cm3 3. 18 (a) We are asked to calculate the unit cell volume for Be. From the solution to Problem 3.7 VC = 6R2c 3 But, c = 1.568a, and a = 2R, or c = 3.14R, and 3 VC = (6)(3.14) R 0.1143 x 10-7 cm] ( )[ 3 = (6) (3.14 ) 3 3 = 4.87 x 10−23 cm3 /unit cell (b) The density of Be is determined as follows: ρ = For HCP, n = 6 atoms/unit cell, and for Be, A ρ = nA Be VC NA Be = 9.01 g/mol. Thus, (6 atoms/unit cell)(9.01 g/mol) 23 -23 3 4.87 x 10 cm /unit cell 6.023 x 10 atoms/mol ( ) ( 23 )
- 26. = 1.84 g/cm3 3 The value given in the literature is 1.85 g/cm . 3.19 This problem calls for us to compute the atomic radius for Mg. In order to do this we must use Equation (3.5), as well as the expression which relates the atomic radius to the unit cell volume for HCP; from Problem 3.7 it was shown that VC = 6R2c 3 In this case c = 1.624(2R). Making this substitution into the previous equation, and then solving for R using Equation (3.5) yields ⎡ ⎤ nAMg ⎥ R = ⎢ ⎢( 1.624) 12 3 ρN A ⎥ ⎣ ⎦ ( 1/3 ) ⎡ (6 atoms/unit cell)(24.31 g/mol ) ⎢ = ⎢ 1.624) 12 3 1.74 g/cm3 6.023 x 10 23 atoms/mol ⎢( ⎣ ( )( ) ( 1/3 ⎤ ⎥ ⎥ ⎥ ⎦ ) = 1.60 x 10-8 cm = 0.160 nm 3.20 This problem asks that we calculate the unit cell volume for Co which has an HCP crystal structure. In order to do this, it is necessary to use a result of Problem 3.7, that is VC = 6R2c 3 The problem states that c = 1.623a, and a = 2R. Therefore VC = (1.623)(12 3 ) R 3 ( = (1.623)(12 3 ) 1.253 x 10 -8 cm ) 3 = 6.64 x 10 24 -23 cm 3 = 6.64 x 10 -2 3 nm
- 27. 3.21 (a) The unit cell shown in the problem belongs to the tetragonal crystal system since a = b = 0.35 nm, c = 0.45 nm, and α = β = γ = 90°. (b) The crystal structure would be called body-centered tetragonal. (c) As with BCC, n = 2 atoms/unit cell. Also, for this unit cell ( VC = 3.5 x 10 −8 = 5.51 x 10 cm −23 ) (4.5 x 10−8 cm) 2 3 cm /unit cell Thus, ρ = = nA VC NA (2 atoms/unit cell)(141 g/mol ) -23 3 23 5.51 x 10 cm /unit cell 6.023 x 10 atoms/mol ( ) ( ) = 8.50 g/cm3 3.22 First of all, open ‘Notepad” in Windows. Now enter into “Notepad” commands to generate the AuCu3 unit cell. One set of commands that may be used is as follows: [DisplayProps] Rotatez=-30 Rotatey=-15 [AtomProps] Gold=LtRed,0.14 Copper=LtYellow,0.13 [BondProps] SingleSolid=LtGray [Atoms] Au1=1,0,0,Gold Au2=0,0,0,Gold Au3=0,1,0,Gold Au4=1,1,0,Gold Au5=1,0,1,Gold Au6=0,0,1,Gold 25
- 28. Au7=0,1,1,Gold Au8=1,1,1,Gold Cu1=0.5,0,0.5,Copper Cu2=0,0.5,0.5,Copper Cu3=0.5,1,0.5,Copper Cu4=1,0.5,0.5,Copper Cu5=0.5,0.5,1,Copper Cu6=0.5,0.5,0,Copper [Bonds] B1=Au1,Au5,SingleSolid B2=Au5,Au6,SingleSolid B3=Au6,Au2,SingleSolid B4=Au2,Au1,SingleSolid B5=Au4,Au8,SingleSolid B6=Au8,Au7,SingleSolid B7=Au7,Au3,SingleSolid B8=Au3,Au4,SingleSolid B9=Au1,Au4,SingleSolid B10=Au8,Au5,SingleSolid B11=Au2,Au3,SingleSolid B12=Au6,Au7,SingleSolid Under the "File" menu of "Note Pad," click "Save As", and then assign the file for this figure a name followed by a period and "mdf"; for example, “AuCu3.mdf”. And, finally save this file in the “mdf” file inside of the “Interactive MSE” folder (which may be found in its installed location). Now, in order to view the unit cell just generated, bring up “Interactive MSE”, and then open any one of the three submodules under “Crystallinity and Unit Cells” or the “Ceramic Structures” module. Next select “Open” under the “File” menu, and then open the “mdf” folder. Finally, select the name you assigned to the item in the window that appears, and hit the “OK” button. The image that you generated will now be displayed. 3.23 First of all, open ‘Notepad” in Windows.. Now enter into “Notepad” commands to generate the AuCu unit cell. One set of commands that may be used is as follows: [DisplayProps] Rotatez=-30 Rotatey=-15 [AtomProps] Gold=LtRed,0.14 Copper=LtYellow,0.13 [BondProps] SingleSolid=LtGray [Atoms] Au1=0,0,0,Gold Au2=1,0,0,Gold Au3=1,1,0,Gold Au4=0,1,0,Gold Au5=0,0,1.27,Gold Au6=1,0,1.27,Gold 26
- 29. Au7=1,1,1.27,Gold Au8=0,1,1.27,Gold Cu1=0.5,0.5,0.635,Copper [Bonds] B1=Au1,Au2,SingleSolid B2=Au2,Au3,SingleSolid B3=Au3,Au4,SingleSolid B4=Au1,Au4,SingleSolid B5=Au5,Au6,SingleSolid B6=Au6,Au7,SingleSolid B7=Au7,Au8,SingleSolid B8=Au5,Au8,SingleSolid B9=Au1,Au5,SingleSolid B10=Au2,Au6,SingleSolid B11=Au3,Au7,SingleSolid B12=Au4,Au8,SingleSolid Under the "File" menu of "Note Pad," click "Save As", and then assign the file for this figure a name followed by a period and "mdf"; for example, “AuCu.mdf”. And, finally save this file in the “mdf” file inside of the “Interactive MSE” folder (which may be found in its installed location). Now, in order to view the unit cell just generated, bring up “Interactive MSE”, and then open any one of the three submodules under “Crystallinity and Unit Cells” or the “Ceramic Structures” module. Next select “Open” under the “File” menu, and then open the “mdf” folder. Finally, select the name you assigned to the item in the window that appears, and hit the “OK” button. The image that you generated will now be displayed. 3.24 A unit cell for the face-centered orthorhombic crystal structure is presented below. 3.25 This problem asks that we list the point coordinates for all of the atoms that are associated with the FCC unit cell. From Figure 3.1b, the atom located of the origin of the unit cell has the coordinates 27
- 30. 000. Coordinates for other atoms in the bottom face are 100, 110, 010, and 11 2 2 0. (The z coordinate for all these points is zero.) 11 For the top unit cell face, the coordinates are 001, 101, 111, 011, and 2 2 1. (These coordinates are the same as bottom-face coordinates except that the “0” z coordinate has been replaced by a “1”.) Coordinates for only those atoms that are positioned at the centers of both side faces, and centers of both front and back faces need to be specified. For the front and back-center face atoms, the coordinates are 1 11 22 and 0 the respective coordinates are 1 1 , respectively. While for the left and right side center-face atoms, 22 1 1 2 0 2 and 1 1 1 . 2 2 3.26 (a) Here we are asked list point coordinates for both sodium and chlorine ions for a unit cell of the sodium chloride crystal structure, which is shown in Figure 12.2. In Figure 12.2, the chlorine ions are situated at all corners and face-centered positions. Therefore, point coordinates for these ions are the same as for FCC, as presented in the previous problem—that is, 000, 100, 110, 010, 001, 101, 111, 011, 11 2 2 0, 11 2 2 1, 1 11 22 , 0 1 1 22 , 1 2 0 1 2 , and 1 1 1 . 2 2 Furthermore, the sodium ions are situated at the centers of all unit cell edges, and, in addition, at the unit cell center. For the bottom face of the unit cell, the point coordinates are as follows: 1 2 1 1 2 2 00 , 1 0 , 1 10 , 0 0 . While, for the horizontal plane that passes through the center of 2 1 1 111 2 2 2 22 the unit cell (which includes the ion at the unit cell center), the coordinates are 0 0 , 1 0 , 1 1 1 2 2 2 11 , and 01 . And for the four ions on the top face 1 1 2 2 01 , 1 1 , , 1 11 , and 0 1 . 2 (b) This portion of the problem calls for us to list the point coordinates of both the zinc and sulfur atoms for a unit cell of the zinc blende structure, which is shown in Figure 12.4. First of all, the sulfur atoms occupy the face-centered positions in the unit cell, which from the solution to Problem 3.25, are as follows: 000, 100, 110, 010, 001, 101, 111, 011, 1 11 22 ,0 1 1 22 , 1 2 0 1 2 , and 11 2 2 0, 11 2 2 1, 1 1 1 . 2 2 Now, using an x-y-z coordinate system oriented as in Figure 3.4, the coordinates of the zinc atom that lies toward the lower-left-front of the unit cell has the coordinates situated toward the lower-right-back of the unit cell has coordinates of that resides toward the upper-left-back of the unit cell has the 3 1 1 4 44 13 1 4 44 113 4 44 , whereas the atom . Also, the zinc atom coordinates. coordinates of the final zinc atom, located toward the upper-right-front of the unit cell, are 28 And, the 3 33 4 44 .
- 31. 3.27 A tetragonal unit in which are shown the 11 1 2 and 111 2 42 point coordinates is presented below. 3.28 This portion of the problem calls for us to draw a [12 1 ] direction within an orthorhombic unit cell (a ≠ b ≠ c, α = β = γ = 90°). Such a unit cell with its origin positioned at point O is shown below. We first move along the +x-axis a units (from point O to point A), then parallel to the +y-axis 2b units (from point A to point B). Finally, we proceed parallel to the z-axis -c units (from point B to point C). The [12 1 ] direction is the vector from the origin (point O) to point C as shown. We are now asked to draw a (210) plane within an orthorhombic unit cell. First remove the three indices from the parentheses, and take their reciprocals--i.e., 1/2, 1, and ∞. This means that the 29
- 32. plane intercepts the x-axis at a/2, the y-axis at b, and parallels the z-axis. The plane that satisfies these requirements has been drawn within the orthorhombic unit cell below. 3.29 (a) This portion of the problem asks that a [0 1 1] direction be drawn within a monoclinic unit cell (a ≠ b ≠ c, and α = β = 90° ≠ γ). One such unit cell with its origin at point O is sketched below. For this direction, there is no projection along the x-axis since the first index is zero; thus, the direction lies in the y-z plane. We next move from the origin along the minus y-axis b units (from point O to point R). Since the final index is a one, move from point R parallel to the z-axis, c units (to point P). Thus, the [0 1 1] direction corresponds to the vector passing from the origin to point P, as indicated in the figure. 30
- 33. (b) A (002) plane is drawn within the monoclinic cell shown below. We first remove the parentheses and take the reciprocals of the indices; this gives ∞, ∞, and 1/2. Thus, the (002) plane parallels both x- and y-axes, and intercepts the z-axis at c/2, as indicated in the drawing. 3.30 (a) We are asked for the indices of the two directions sketched in the figure. For direction 1, the projection on the x-axis is zero (since it lies in the y-z plane), while projections on the y- and z-axes are b/2 and c, respectively. This is an [012] direction as indicated in the summary below x Projections y z 0a b/2 c 0 1/2 1 0 1 2 Projections in terms of a, b, and c Reduction to integers Enclosure [012] Direction 2 is [11 2 ] as summarized below. x Projections y z a/2 b/2 -c 1/2 1/2 -1 1 1 -2 Projections in terms of a, b, and c Reduction to integers 31
- 34. Enclosure [11 2 ] (b) This part of the problem calls for the indices of the two planes which are drawn in the sketch. Plane 1 is an (020) plane. The determination of its indices is summarized below. x y z ∞a b/2 ∞c Intercepts in terms of a, b, and c ∞ 1/2 ∞ Reciprocals of intercepts 0 2 0 Intercepts Enclosure (020) Plane 2 is a (2 2 1) plane, as summarized below. x y z Intercepts a/2 -b/2 c Intercepts in terms of a, b, and c 1/2 -1/2 1 2 -2 1 Reciprocals of intercepts Enclosure (2 2 1) 3.31 The directions asked for are indicated in the cubic unit cells shown below. 32
- 35. 3.32 Direction A is a [ 1 10] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections y z -a b 0c -1 1 0 Projections in terms of a, b, and c Reduction to integers not necessary Enclosure [ 1 10] Direction B is a [121] direction, which determination is summarized as follows. The vector passes through the origin of the coordinate system and thus no translation is necessary. Therefore, x Projections y a b 2 Projections in terms of a, b, 33 z c 2
- 36. and c Reduction to integers 1 1 1 2 1 2 2 Enclosure 1 [121] Direction C is a [0 1 2 ] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x y b 0a − and c 0 - Reduction to integers 0 z -1 Projections 2 -c Projections in terms of a, b, Enclosure 1 -1 2 -2 [0 1 2 ] Direction D is a [12 1] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections y a z c -b 2 2 Projections in terms of a, b, and c Reduction to integers 1 1 -1 2 1 2 -2 Enclosure 1 [12 1] 3.33 Direction A is a [33 1 ] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections y a b Projections in terms of a, b, 34 z - c 3
- 37. and c 1 1 Reduction to integers 3 3 Enclosure - 1 3 -1 [33 1 ] Direction B is a [4 03 ] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections y 2a - z c - 0 - 0 3 0b -3 2 Projections in terms of a, b, and c Reduction to integers - 2 3 -4 Enclosure 1 2 [4 03 ] Direction C is a [3 61] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections - y a z c b 2 6 Projections in terms of a, b, and c - Reduction to integers 1 1 1 2 -3 6 6 Enclosure 1 [3 61] Direction D is a [ 1 1 1 ] direction, which determination is summarized as follows. We first of all position the origin of the coordinate system at the tail of the direction vector; then in terms of this new coordinate system x Projections - y a b 2 2 Projections in terms of a, b, 35 z - c 2
- 38. 1 1 2 2 -1 and c 1 - Reduction to integers Enclosure - 1 2 -1 [111] 3.34 For tetragonal crystals a = b ≠ c and α = β = γ = 90°; therefore, projections along the x and y axes are equivalent, which are not equivalent to projections along the z axis. (a) Therefore, for the [011] direction, equivalent directions are the following: [101], [ 1 0 1] , [ 1 01 ] , [10 1] , [01 1 ] , [0 1 1] , and [0 1 1 ] . (b) Also, for the [100] direction, equivalent directions are the following: [ 1 00] , [010], and [0 1 0 ] . 3.35 (a) We are asked to convert [100] and [111] directions into the four- index Miller-Bravais scheme for hexagonal unit cells. For [100] u' = 1, v' = 0, w' = 0 From Equations (3.6) u = 2n n n (2 − 0) = (2u ' − v ' ) = 3 3 3 v = n n n (0 − 1) = (2v ' − u' ) = 3 3 3 n ⎛ 2n n ⎞ t = - (u + v) = - ⎜ − ⎟=3⎠ ⎝ 3 3 w = nw' = 0 If we let n = 3, then u = 2, v = -1, t = -1, and w = 0. Thus, the direction is represented as [uvtw] = [2 1 1 0 ] . For [111], u' = 1, v' = 1, and w' = 1; therefore, u = v = n n (2 − 1) = 3 3 n n (2 − 1) = 3 3 36
- 39. 2n ⎛n n⎞ t =-⎜ + ⎟= ⎝ 3 3⎠ 3 w=n If we again let n = 3, then u = 1, v = 1, t = -2, and w = 3. Thus, the direction is represented as [11 2 3] . (b) This portion of the problem asks for the same conversion of the (010) and (101) planes. A plane for hexagonal is represented by (hkil) where i = - (h + k), and h, k, and l are the same for both systems. For the (010) plane, h = 0, k = 1, l = 0, and i = - (0 + 1) = -1 Thus, the plane is now represented as (hkil) = (01 1 0) . For the (101) plane, i = - (1 + 0) = -1, and (hkil) = (10 1 1) . 3.36 For plane A we will leave the origin at the unit cell as shown. If we extend this plane back into the plane of the page, then it is a (11 1 ) plane, as summarized below. x Intercepts y z a b -c 1 1 -1 1 1 -1 Intercepts in terms of a, b, and c Reciprocals of intercepts Reduction not necessary Enclosure (11 1 ) For plane B we will leave the origin of the unit cell as shown; this is a (230) plane, as summarized below. x Intercepts y z a b 2 3 ∞c Intercepts in terms of a, b, 37
- 40. and c Reciprocals of intercepts 1 1 2 3 2 3 Enclosure ∞ 0 (230) 3.37 For plane A we will move the origin of the coordinate system one unit cell distance to the right along the y axis; thus, this is a (1 1 0 ) plane, as summarized below. x Intercepts y a - 2 z b ∞c 2 Intercepts in terms of a, b, and c 1 - 2 1 2 ∞ Reciprocals of intercepts 2 -2 0 Reduction 1 -1 0 Enclosure (1 1 0 ) For plane B we will leave the origin of the unit cell as shown; thus, this is a (122) plane, as summarized below. x Intercepts y b c 2 2 1 1 2 2 2 a z 2 Intercepts in terms of a, b, and c Reciprocals of intercepts 1 1 Reduction not necessary Enclosure (122) 3.38 For plane A since the plane passes through the origin of the coordinate system as shown, we will move the origin of the coordinate system one unit cell distance vertically along the z axis; thus, this is a (21 1 ) plane, as summarized below. 38
- 41. x Intercepts y b -1 1 2 -c 1 a z -1 Intercepts in terms of a, b, and c Reciprocals of intercepts 1 2 2 Reduction not necessary Enclosure (21 1 ) For plane B, since the plane passes through the origin of the coordinate system as shown, we will move the origin one unit cell distance vertically along the z axis; this is a (02 1 ) plane, as summarized below. x Intercepts y ∞a b 2 z -c Intercepts in terms of a, b, and c Reciprocals of intercepts 1 ∞ 2 0 2 Reduction -1 not necessary Enclosure -1 (02 1 ) 3.39 The (01 1 1) and (2 1 1 0 ) planes in a hexagonal unit cell are shown below. 39
- 42. 3.40 (a) For this plane we will leave the origin of the coordinate system as shown; thus, this is a (12 11) plane, as summarized below. a1 Intercepts a - Intercepts in terms of a's and c 1 - Reciprocals of intercepts 1 a3 2 1 1 -2 2 1 c 1 a z a a2 1 Reduction not necessary Enclosure (12 11) (b) For this plane we will leave the origin of the coordinate system as shown; thus, this is a (2 1 1 2) plane, as summarized below. a1 a2 a3 z Intercepts a/2 -a -a c/2 Intercepts in terms of a's and c 1/2 -1 -1 1/2 2 -1 -1 2 Reciprocals of intercepts Reduction not necessary Enclosure (2 1 1 2) 3.41 The planes called for are plotted in the cubic unit cells shown below. 40
- 43. 3.42 (a) The atomic packing of the (100) plane for the FCC crystal structure is called for. An FCC unit cell, its (100) plane, and the atomic packing of this plane are indicated below. (b) For this part of the problem we are to show the atomic packing of the (111) plane for the BCC crystal structure. A BCC unit cell, its (111) plane, and the atomic packing of this plane are indicated below. 41
- 44. 3.43 (a) The unit cell in Problem 3.21 is body-centered tetragonal. Only the (100) (front face) and (0 1 0) (left side face) planes are equivalent since the dimensions of these planes within the unit cell (and therefore the distances between adjacent atoms) are the same (namely 0.45 nm x 0.35 nm), which are different than the (001) (top face) plane (namely 0.35 nm x 0.35 nm). (b) The equivalent planes are (101), (011), and (1 01) ; the dimensions of these planes within the [ unit cell are the same--that is 0.35 nm x (0.35 nm) 2 + (0.45 nm)2 ] 1/ 2 . (c) All of the (111), (1 1 1) , (11 1) , and ( 1 1 1 ) planes are equivalent. 3.44 (a) The intersection between (110) and (111) planes results in a [ 1 10] , or equivalently, a [1 1 0] direction. (b) The intersection between (110) and (1 1 0) planes results in a [001], or equivalently, a [00 1 ] direction. (c) The intersection between (11 1 ) and (001) planes results in a [ 1 10] , or equivalently, a [1 1 0] direction. 3.45 (a) In the figure below is shown a [100] direction within an FCC unit cell. For this [100] direction there is one atom at each of the two unit cell corners, and, thus, there is the equivalent of 1 atom that is centered on the direction vector. The length of this direction vector is just the unit cell edge length, 2R 2 [Equation (3.1)]. Therefore, the expression for the linear density of this plane is LD100 = number of atoms centered on [100] direction vector length of [100] direction vector = 1 atom 1 = 2R 2 2R 2 An FCC unit cell within which is drawn a [111] direction is shown below. 42
- 45. For this [111] direction, the vector shown passes through only the centers of the single atom at each of its ends, and, thus, there is the equivalence of 1 atom that is centered on the direction vector. The length of this direction vector is denoted by z in this figure, which is equal to z= 2 2 x +y where x is the length of the bottom face diagonal, which is equal to 4R. Furthermore, y is the unit cell edge length, which is equal to 2R 2 [Equation (3.1)]. Thus, using the above equation, the length z may be calculate as follows: z= (4R)2 ( + 2R 2 ) 2 = 24R2 = 2R 6 Therefore, the expression for the linear density of this plane is LD111 = number of atoms centered on [111] direction vector length of [111] direction vector = 1 atom 1 = 2R 6 2R 6 (b) From the table inside the front cover, the atomic radius for copper is 0.128 nm. Therefore, the linear density for the [100] direction is LD100 (Cu) = 1 1 −1 −9 −1 = = 2.76 nm = 2.76 x 10 m 2R 2 (2)(0.128 nm) 2 While for the [111] direction 43
- 46. LD111(Cu) = 1 1 −1 −9 −1 = = 1.59 nm = 1.59 x 10 m 2R 6 (2)(0.128 nm) 6 3.46 (a) In the figure below is shown a [110] direction within a BCC unit cell. For this [110] direction there is one atom at each of the two unit cell corners, and, thus, there is the equivalence of 1 atom that is centered on the direction vector. The length of this direction vector is denoted by x in this figure, which is equal to x= 2 2 z −y where y is the unit cell edge length, which, from Equation (3.3) is equal to 4R . Furthermore, z is 3 the length of the unit cell diagonal, which is equal to 4R Thus, using the above equation, the length x may be calculate as follows: x = (4R)2 ⎛ 4R ⎞ 2 − ⎜ ⎟ = ⎝ 3⎠ 2 32R 3 = 4R 2 3 Therefore, the expression for the linear density of this direction is LD110 = number of atoms centered on [110] direction vector length of [110] direction vector = 1 atom 4R 2 3 = 3 4R 2 A BCC unit cell within which is drawn a [111] direction is shown below. 44
- 47. For although the [111] direction vector shown passes through the centers of three atoms, there is an equivalence of only two atoms associated with this unit cell—one-half of each of the two atoms at the end of the vector, in addition to the center atom belongs entirely to the unit cell. Furthermore, the length of the vector shown is equal to 4R, since all of the atoms whose centers the vector passes through touch one another. Therefore, the linear density is equal to LD111 = number of atoms centered on [111] direction vector length of [111] direction vector = 2 atoms 1 = 4R 2R (b) From the table inside the front cover, the atomic radius for iron is 0.124 nm. Therefore, the linear density for the [110] direction is LD110 (Fe) = 3 4R 2 = 3 (4)(0.124 nm) 2 = 2.47 nm−1 = 2.47 x 10 −9 m−1 While for the [111] direction LD111(Fe) = 1 1 = = 4.03 nm−1 = 4.03 x 10−9 m−1 2R (2)(0.124 nm) 3.47 (a) In the figure below is shown a (100) plane for an FCC unit cell. 45
- 48. For this (100) plane there is one atom at each of the four cube corners, each of which is shared with four adjacent unit cells, while the center atom lies entirely within the unit cell. Thus, there is the equivalence of 2 atoms associated with this FCC (100) plane. The planar section represented in the above figure is a square, wherein the side lengths are equal to the unit cell edge length, 2R 2 ( [Equation (3.1)]; and, thus, the area of this square is just 2 R 2 )2 = 8R2. Hence, the planar density for this (100) plane is just PD100 = number of atoms centered on (100) plane area of (100) plane = 2 atoms 8 R2 = 1 4R 2 That portion of an FCC (111) plane contained within a unit cell is shown below. There are six atoms whose centers lie on this plane, which are labeled A through F. One-sixth of each of atoms A, D, and F are associated with this plane (yielding an equivalence of one-half atom), with one-half of each of atoms B, C, and E (or an equivalence of one and one-half atoms) for a total equivalence of two atoms. Now, the area of the triangle shown in the above figure is equal to onehalf of the product of the base length and the height, h. If we consider half of the triangle, then 46
- 49. (2R)2 + h 2 = (4R)2 which leads to h = 2 R 3 . Thus, the area is equal to Area = ( ) 4R(h) (4R) 2R 3 2 = 4R = 2 2 3 And, thus, the planar density is number of atoms centered on (111) plane area of (111) plane PD111 = = 2 atoms = 4R 2 3 1 2R2 3 (b) From the table inside the front cover, the atomic radius for aluminum is 0.143 nm. Therefore, the planar density for the (100) plane is PD100 (Al) = 1 4 R2 = 1 4(0.143 nm)2 = 12.23 nm−2 = 1.223 x 10 −17 m−2 While for the (111) plane PD111(Al) = 1 2R2 3 = 1 2 3 (0.143 nm) 2 = 14.12 nm−2 = 1.412 x 10 −17 m−2 3.48 (a) A BCC unit cell within which is drawn a [100] plane is shown below. For this (100) plane there is one atom at each of the four cube corners, each of which is shared with four adjacent unit cells. Thus, there is the equivalence of 1 atom associated with this BCC (100) plane. The planar section represented in the above figure is a square, wherein the side lengths are 47
- 50. equal to the unit cell edge length, ⎛ 4R ⎞ ⎜ ⎟ ⎝ 3⎠ 2 = 4R [Equation (3.3)]; and, thus, the area of this square is just 3 16 R 2 . Hence, the planar density for this (100) plane is just 3 PD100 = number of atoms centered on (100) plane area of (100) plane = 1 atom 16 R2 = 3 16 R2 3 A BCC unit cell within which is drawn a [110] plane is shown below. For this (110) plane there is one atom at each of the four cube corners through which it passes, each of which is shared with four adjacent unit cells, while the center atom lies entirely within the unit cell. Thus, there is the equivalence of 2 atoms associated with this BCC (110) plane. The planar section represented in the above figure is a rectangle, as noted in the figure below. 48
- 51. From this figure, the area of the rectangle is the product of x and y. The length x is just the unit cell 4R . Now, the diagonal length z is equal to 4R. For 3 edge length, which for BCC [Equation (3.3)] is the triangle bounded by the lengths x, y, and z y= 2 2 z −x Or y = ⎛ 4R ⎞ 2 4R 2 (4R) − ⎜ ⎟ = 3 ⎝ 3⎠ 2 Thus, in terms of R, the area of this (110) plane is just ⎛ 4 R ⎞ ⎛ 4R 2 ⎞ 16R2 ⎟ = ⎟⎜ Area(110) = xy = ⎜ 3 3 ⎠ ⎝ 3⎠⎝ 2 And, finally, the planar density for this (110) plane is just PD110 = number of atoms centered on (110) plane area of (110) plane = 2 atoms 16R2 2 = 3 8R 2 2 3 (b) From the table inside the front cover, the atomic radius for molybdenum is 0.136 nm. Therefore, the planar density for the (100) plane is PD100 (Mo) = 3 16R2 = 3 16(0.136 nm)2 = 10.14 nm−2 = 1.014 x 10−17 m −2 While for the (110) plane PD110 (Mo) = 3 8R 2 2 = 3 8 (0.136 nm) 2 2 = 14.34 nm−2 = 1.434 x 10−17 m −2 3.49 (a) A (0001) plane for an HCP unit cell is show below. 49
- 52. Each of the 6 perimeter atoms in this plane is shared with three other unit cells, whereas the center atom is shared with no other unit cells; this gives rise to three equivalent atoms belonging to this plane. In terms of the atomic radius R, the area of each of the 6 equilateral triangles that have been 2 drawn is R 3 , or the total area of the plane shown is 6R 2 3 . And the planar density for this (0001) plane is equal to PD0001 = number of atoms centered on (0001) plane area of (0001) plane = 3 atoms 6R2 3 = 1 2R2 3 (b) From the table inside the front cover, the atomic radius for titanium is 0.145 nm. Therefore, the planar density for the (0001) plane is PD0001(Ti) = 1 2R2 3 = 1 2 3 (0.145 nm) 2 = 13.73 nm−2 = 1.373 x 10 −17 m −2 3.50 Unit cells are constructed below from the three crystallographic planes provided in the problem. 50
- 53. (a) This unit cell belongs to the tetragonal system since a = b = 0.40 nm, c = 0.55 nm, and α = β = γ = 90°. (b) This crystal structure would be called body-centered tetragonal since the unit cell has tetragonal symmetry, and an atom is located at each of the corners, as well as the cell center. 3.51 The unit cells constructed below show the three crystallographic planes that were provided in the problem. (a) This unit cell belongs to the orthorhombic crystal system since a = 0.25 nm, b = 0.30 nm, c = 0.20 nm, and α = β = γ = 90°. (b) This crystal structure would be called face-centered orthorhombic since the unit cell has orthorhombic symmetry, and an atom is located at each of the corners, as well as at each of the face centers. (c) In order to compute its atomic weight, we employ Equation (3.5), with n = 4; thus 51
- 54. A = ρVCN A n (18.91 g/cm3 )(2.0)(2.5)(3.0) (x 10-24 cm3 /unit cell)(6.023 x 1023 atoms/mol) = 4 atoms/unit cell = 42.7 g/mol 3.52 Although each individual grain in a polycrystalline material may be anisotropic, if the grains have random orientations, then the solid aggregate of the many anisotropic grains will behave isotropically. 3.53W From the table, aluminum has an FCC crystal structure and an atomic radius of 0.1431 nm. Using Equation (3.1), the lattice parameter a may be computed as a = 2 R 2 = (2)(0.1431 nm) 2 = 0.4048 nm Now, the interplanar spacing d110 maybe determined using Equation (3.3W) as d110 = a 2 (1) 2 + (1) 2 = + (0) 0.4048 nm = 0.2862 nm 2 3.54W We must first calculate the lattice parameter using Equation (3.3) and the value of R cited in Table 3.1 as 4R a= 3 = (4)(0.1249 nm) 3 = 0.2884 nm Next, the interplanar spacing may be determined using Equation (3.3W) according to d 310 = a 2 (3) 2 + (1) 2 = + (0) And finally, employment of Equation (3.2W) yields 52 0.2884 nm = 0.0912 nm 10
- 55. sin θ = nλ (1)(0.0711 nm) = = 0.390 2d (2)(0.0912 nm) θ = sin-1(0.390) = 22.94° And 2θ = (2)(22.94°) = 45.88° 3.55W From the table, α-iron has a BCC crystal structure and an atomic radius of 0.1241 nm. Using Equation (3.3) the lattice parameter, a, may be computed as a= 4R 3 = (4)(0.1241 nm) 3 = 0.2866 nm Now, the d111 interplanar spacing may be determined using Equation (3.3W) as a d111 = 2 (1) 2 + (1) 2 = 0.2866 nm = 0.1655 nm 3 = 0.2866 nm = 0.1170 nm 6 + (1) And, similarly for d211 a d 211 = (2)2 + (1)2 + (1)2 3.56W (a) From the data given in the problem, and realizing that 36.12° = 2θ, the interplanar spacing for the (311) set of planes may be computed using Equation (3.3W) as d 311 = nλ (1)(0.0711 nm) = = 0.1147 nm 2 sin θ 36.12° ⎞ ⎛ (2) ⎜ sin ⎟ 2 ⎠ ⎝ (b) In order to compute the atomic radius we must first determine the lattice parameter, a, using Equation (3.3W), and then R from Equation (3.1) since Rh has an FCC crystal structure. Therefore, 2 a = d 311 (3) 2 + (1) 2 + (1) = (0.1147 nm) 53 ( 11)= 0.3804 nm
- 56. And R = a 0.3804 nm = = 0.1345 nm 2 2 2 2 3.57W. (a) From the data given in the problem, and realizing that 75.99° = 2θ, the interplanar spacing for the (211) set of planes may be computed using Equation (3.2W) as d 211 = nλ (1)(0.1659 nm) = = 0.1348 nm 2 sin θ 75.99°⎞ ⎛ (2)⎜ sin ⎟ 2 ⎠ ⎝ (b) In order to compute the atomic radius we must first determine the lattice parameter, a, using Equation (3.3W), and then R from Equation (3.3) since Nb has a BCC crystal structure. Therefore, 2 2 a = d 211 (2) + (1) 2 + (1) = (0.1347 nm) ( 6 ) = 0.3300 nm And R= a 3 (0.3300 nm) 3 = = 0.1429 nm 4 4 3.58W The first step to solve this problem is to compute the interplanar spacing using Equation (3.2W). Thus, d hkl (1)(0.1542 nm) nλ = 0.2035 nm = ⎛ 44.53° ⎞ 2 sin θ (2)⎜ sin ⎟ ⎝ 2 ⎠ Now, employment of both Equations (3.3W) and (3.1), and the value of R for nickel from Table 3.1 (0.1246 nm) leads to h 2 + k 2 2 + l = a d hkl = (2)(0.1246 nm) 2 (0.2035 nm) This means that 54 = 2R 2 d hkl = 1.732
- 57. h2 + k2 + l2 = (1.732)2 = 3.0 By trial and error, the only three integers which are all odd or even, the sum of the squares of which equals 3.0 are 1, 1, and 1. Therefore, the set of planes responsible for this diffraction peak is the (111) set. 3.59W For each peak, in order to compute the interplanar spacing and the lattice parameter we must employ Equations (3.3W) and (3.2W), respectively. For the first peak which occurs at 31.3° d111 = nλ (1)(0.1542 nm) = = 0.2858 nm 2 sin θ 31.3° ⎞ ⎛ (2)⎜ sin ⎟ 2 ⎠ ⎝ And a = dhkl (h)2 + (k)2 + (l)2 = d111 (1)2 + (1)2 + (1)2 = (0.2858 nm) 3 = 0.4950 nm Similar computations are made for the other peaks which results are tabulated below: Peak Index 2θ dhkl(nm) a (nm) 200 36.6 0.2455 0.4910 220 52.6 0.1740 0.4921 311 62.5 0.1486 0.4929 222 65.5 0.1425 0.4936 3.60W The first four diffraction peaks that will occur for BCC consistent with h + k + l being even are (110), (200), (211), and (220). 3.61W (a) Since W has a BCC crystal structure, only those peaks for which h + k + l are even will appear. Therefore, the first peak results by diffraction from (110) planes. (b) For each peak, in order to calculate the interplanar spacing we must employ Equation (3.2W). For the first peak which occurs at 40.2° 55
- 58. d110 = nλ (1)(0.1542 nm) = = 0.2244 nm 2 sin θ 40.2° ⎞ ⎛ (2)⎜ sin ⎟ 2 ⎠ ⎝ (c) Employment of Equations (3.3W) and (3.3) is necessary for the computation of R for W as R = = a 3 4 (dhkl )( 3) = (0.2244 nm)( 3 ) (h)2 + (k)2 + (l) 2 4 (1)2 + (1)2 + (0)2 4 = 0.1374 nm 3.62 A material in which atomic bonding is predominantly ionic in nature is less likely to form a noncrystalline solid upon solidification than a covalent material because covalent bonds are directional whereas ionic bonds are nondirectional; it is more difficult for the atoms in a covalent material to assume positions giving rise to an ordered structure. 56
- 59. CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS 4.1 In order to compute the fraction of atom sites that are vacant in lead at 600 K, we must employ Equation (4.1). As stated in the problem, Q = 0.55 eV/atom. Thus, v ⎡ ⎤ ⎛ Q ⎞ 0.55 eV / atom ⎢ ⎥ = exp ⎜ − V ⎟ = exp ⎢− −5 eV / atom -K (600 K) ⎥ N kT ⎠ ⎝ ⎢ 8.62 x 10 ⎥ ⎣ ⎦ NV ( ) = 2.41 x 10 -5 4.2 Determination of the number of vacancies per cubic meter in gold at 900°C (1173 K) requires the utilization of Equations (4.1) and (4.2) as follows: NA ρ Au ⎛ Q ⎞ ⎛ Q ⎞ exp ⎜ − V ⎟ NV = N exp ⎜ − V ⎟ = AAu ⎝ kT ⎠ ⎝ kT ⎠ = 19.32 (6.023 x 10 23 atoms/ mol)( g / cm3 )exp ⎢⎡− ⎢ ⎢ ⎣ 196.9 g / mol ⎤ ⎥ −5 eV / atom − K (1173 K) ⎥ 8.62 x 10 ⎥ ⎦ ( 0.98 eV / atom ) = 3.65 x 1018 cm-3 = 3.65 x 1024 m-3 4.3 This problem calls for the computation of the energy for vacancy formation in silver. Upon examination of Equation (4.1), all parameters besides Q are given except N, the total number of v atomic sites. However, N is related to the density, (ρ), Avogadro's number (N ), and the atomic A weight (A) according to Equation (4.2) as N = = NA ρ Ag A Ag (6.023 x 10 23 atoms / mol)(10.49 g / cm 3 ) 107.87 g / mol 57
- 60. = 5.86 x 1022 atoms/cm3 = 5.86 x 1028 atoms/m3 Now, taking natural logarithms of both sides of Equation (4.1), and, after some algebraic manipulation ⎛ NV ⎞ QV = − RT ln ⎜ ⎟ ⎝ N ⎠ ⎡ 3.60 x 10 23 m−3 ⎤ ⎥ = − 8.62 x 10-5 eV/atom - K (1073 K) ln ⎢ 28 −3 ⎥ ⎢ ⎣ 5.86 x 10 m ⎦ ( ) = 1.11 eV/atom 4.4 In this problem we are asked to cite which of the elements listed form with Cu the three possible solid solution types. For complete substitutional solubility the following criteria must be met: 1) the difference in atomic radii between Cu and the other element (∆R%) must be less than ±15%, 2) the crystal structures must be the same, 3) the electronegativities must be similar, and 4) the valences should be the same, or nearly the same. Below are tabulated, for the various elements, these criteria. Crystal Element ∆R% Cu ∆Electro- Structure negativity FCC Valence 2+ C -44 H -64 O -53 Ag +13 FCC 0 1+ Al +12 FCC -0.4 3+ Co -2 HCP -0.1 2+ Cr -2 BCC -0.3 3+ Fe -3 BCC -0.1 2+ Ni -3 FCC -0.1 2+ Pd +8 FCC +0.3 2+ Pt +9 FCC +0.3 2+ Zn +4 HCP -0.3 2+ 58
- 61. (a) Ni, Pd, and Pt meet all of the criteria and thus form substitutional solid solutions having complete solubility. (b) Ag, Al, Co, Cr, Fe, and Zn form substitutional solid solutions of incomplete solubility. All these metals have either BCC or HCP crystal structures, and/or the difference between their atomic radii and that for Cu are greater than ±15%, and/or have a valence different than 2+. (c) C, H, and O form interstitial solid solutions. These elements have atomic radii that are significantly smaller than the atomic radius of Cu. 4.5 In the drawing below is shown the atoms on the (100) face of an FCC unit cell; the interstitial site is at the center of the edge. The diameter of an atom that will just fit into this site (2r) is just the difference between the unit cell edge length (a) and the radii of the two host atoms that are located on either side of the site (R); that is 2r = a - 2R However, for FCC a is related to R according to Equation (3.1) as a = 2R 2 ; therefore, solving for r gives r = a − 2R 2R 2 − 2R = = 0.41R 2 2 A (100) face of a BCC unit cell is shown below. 59
- 62. The interstitial atom that just fits into this interstitial site is shown by the small circle. It is situated in the plane of this (100) face, midway between the two vertical unit cell edges, and one quarter of the distance between the bottom and top cell edges. From the right triangle that is defined by the three arrows we may write ⎛ a⎞ ⎜ ⎟ ⎝ 2⎠ However, from Equation (3.3), a = ⎛ 4R ⎞ ⎜ ⎟ ⎝2 3⎠ 2 ⎛a⎞ + ⎜ ⎟ ⎝ 4⎠ 2 = (R + r) 2 4R , and, therefore, the above equation takes the form 3 2 ⎛ 4R ⎞ + ⎜ ⎟ ⎝ 4 3⎠ 2 = R2 + 2R r + r 2 After rearrangement the following quadratic equation results: r 2 + 2Rr − 0.667R 2 = 0 And upon solving for r, r = 0.291R. 60
- 63. Thus, for a host atom of radius R, the size of an interstitial site for FCC is approximately 1.4 times that for BCC. 4.6 (a) This problem asks that we derive Equation (4.7a). To begin, C1 is defined according to Equation (4.3) as m1 C1 = m + m 1 x 100 2 or, equivalently ' m1 C1 = ' ' m1 + m2 x 100 where the primed m's indicate masses in grams. From Equation (4.4) we may write ' m1 = nm1 A 1 ' m 2 = nm2 A2 And, substitution into the C1 expression C1 = nm1 A1 x 100 nm1A 1 + nm2 A 2 From Equation (4.5) it is the case that ( m1 + C' n nm1 = 1 m2 ) 100 ( m1 + C' n nm2 = n 2 n m2 ) 100 And substitution of these expressions into the above equation leads to 61
- 64. ' C1A 1 C1 = ' ' C1A 1 + C 2A 2 x 100 which is just Equation (4.7a). '' (b) This problem asks that we derive Equation (4.9a). To begin, C1 is defined as the mass of component 1 per unit volume of alloy, or '' C1 = m1 V If we assume that the total alloy volume V is equal to the sum of the volumes of the two constituents-i.e., V = V1 + V2--then '' C1 = m 1 V + V 1 2 Furthermore, the volume of each constituent is related to its density and mass as V1 = V2 = m1 ρ 1 m2 ρ 2 This leads to '' C1 = m m1 ρ 1 1 + m2 ρ 2 From Equation (4.3), m1 and m2 may be expressed as follows: m1 = ( C1 m1 + m 2 100 62 )
- 65. ( C2 m1 + m2 m2 = ) 100 Substitution of these equations into the preceding expression yields ( '' C1 = ) ) ( C1 m1 + m 2 100 C1 m1 + m2 C 2 m1 + m 2 100 100 + ρ1 ρ2 ( = ) C1 C1 ρ + C2 1 ρ 2 If the densities ρ1 and ρ2 are given in units of g/cm3, then conversion to units of kg/m3 requires that we multiply this equation by 103, inasmuch as 103 g/cm3 = 1 kg/m3 Therefore, the previous equation takes the form '' C1 = C1 C1 ρ + 1 3 C2 ρ x 10 2 which is the desired expression. (c) Now we are asked to derive Equation (4.10a). The density of an alloy ρave is just the total alloy mass M divided by its volume V ρ ave = Or, in terms of the component elements 1 and 2 63 M V
- 66. m1 + m2 ρ ave = V + V 1 2 Here it is assumed that the total alloy volume is equal to the separate volumes of the individual components, which is only an approximation; normally V will not be exactly equal to (V1 + V2). Each of V1 and V2 may be expressed in terms of its mass density, which when substituted into the above equation m1 + m2 ρ ave = m1 ρ + 1 m2 ρ 2 Furthermore, from Equation (4.3) m1 = m2 = ( ) ( ) C1 m1 + m 2 100 C2 m1 + m2 100 Which, when substituted into the above ρave expression yields ρ ave = m1 + m2 (1 C m + m 1 2 ) 100 ρ1 = 2 + (m1 + m 2 ) 100 ρ2 100 C1 ρ1 (d) C + C2 ρ2 And, finally, the derivation of Equation (4.11b) for Aave is requested. The alloy average molecular weight is just the ratio of total alloy mass in grams M' and the total number of moles in the alloy Nm. That is A ave = ' ' m1 + m 2 M' = N n + n m m1 64 m2
- 67. But using Equation (4.4) we may write ' m1 = nm1 A 1 ' m2 = nm2 A 2 Which, when substituted into the above Aave expression yields A ave = M' N n m1 A 1 + nm2 A 2 n + n = m m1 m2 Furthermore, from Equation (4.5) ( m1 + C' n 1 nm1 = n m2 ) 100 ( m1 + C' n 2 nm2 = n m2 ) 100 Thus ( ' C1A 1 nm1 + nm2 100 A ave = )+ n m1 = ( ' C2 A 2 nm1 + n m2 100 + n ) m2 ' ' C1A1 + C 2A 2 100 which is the desired result. 4.7 In order to compute composition, in atom percent, of a 92.5 wt% Ag-7.5 wt% Cu alloy, we employ Equation (4.6) as C 'Ag = C AgA C A Ag Cu Cu +C 65 A Cu Ag x 100
- 68. (92.5)(63.55 g / mol) x 100 (92.5)(63.55 g/ mol) + (7.5)(107.87g / mol) = = 87.9 at% ' CCu = C C A Cu Ag A Ag Cu +C A x 100 Cu Ag (7.5)(107.87 g / mol) x 100 (92.5)(63.55 g/ mol) + (7.5)(107.87g / mol) = = 12.1 at% 4.8 In order to compute composition, in weight percent, of a 5 at% Cu-95 at% Pt alloy, we employ Equation (4.7) as C' A C Cu = Cu Cu C' A Cu Cu = +C' A x 100 Pt Pt (5)(63.55 g / mol) x 100 (5)(63.55 g / mol) + (95)(195.08 g / mol) = 1.68 wt% C' A CPt = Pt Pt C' A Cu Cu = + C' A x 100 Pt Pt (95)(195.08 g / mol) x 100 (5)(63.55 g / mol) + (95)(195.08 g / mol) = 98.32 wt% 4.9 The concentration, in weight percent, of an element in an alloy may be computed using a modification of Equation (4.3). For this alloy, the concentration of iron (C ) is just Fe 66
- 69. mFe CFe = = mFe + mC + mCr x 100 105 kg x 100 = 98.87 wt% 105 kg + 0.2 kg + 1.0 kg Similarly, for carbon CC = 0.2 kg x 100 = 0.19 wt% 105 kg + 0.2 kg + 1.0 kg CCr = 1.0 kg x 100 = 0.94 wt% 105 kg + 0.2 kg + 1.0 kg And for chromium 4.10 The concentration of an element in an alloy, in atom percent, may be computed using Equation (4.5). With this problem, it first becomes necessary to compute the number of moles of both Cu and Zn, for which Equation (4.4) is employed. Thus, the number of moles of Cu is just nm m' Cu = A Cu = Cu 33 g = 0.519 mol 63.55 g / mol Likewise, for Zn nm = Zn 47 g = 0.719 mol 65.39 g / mol Now, use of Equation (4.5) yields n ' C Cu = = m n m Cu Cu +n x 100 m Zn 0.519 mol x 100 = 41.9 at% 0.519 mol + 0.719 mol Also, 67
- 70. 0.719 mol x 100 = 58.1 at% 0.519 mol + 0.719 mol ' C Zn = 4.11 In this problem we are asked to determine the concentrations, in atom percent, of the Ag-Au-Cu alloy. It is first necessary to convert the amounts of Ag, Au, and Cu into grams. ' mAg = (44.5 lbm )(453.6 g/lbm ) = 20,185 g ' mAu = (83.7 lbm )(453.6 g/lb m ) = 37,966 g ' mCu = (5.3 lbm )(453.6 g/lbm ) = 2,404 g These masses must next be converted into moles [Equation (4.4)], as nm ' mAg = AAg Ag nm = 37, 966 g = 192.8 mol 196.97 g / mol = Au nm 20,185 g = 187.1 mol 107.87 g / mol = Cu 2,404 g = 37.8 mol 63.55 g / mol Now, employment of a modified form of Equation (4.5) n m ' C Ag = = +n n m Ag Ag m + n Au x 100 m Cu 187.1 mol x 100 = 44.8 at% 187.1 mol + 192.8 mol + 37.8 mol C 'Au = ' CCu = 192.8 mol x 100 = 46.2 at% 187.1 mol + 192.8 mol + 37.8 mol 37.8 mol x 100 = 9.0 at% 187.1 mol + 192.8 mol + 37.8 mol 68
- 71. 4.12 We are asked to compute the composition of an alloy in atom percent. Employment of Equation (4.6) leads to ' CPb = = CPb ASn CPb ASn + CSn APb x 100 5.5(118.69 g / mol) x 100 5.5 (118.69 g / mol) + 94.5(207.2 g / mol) = 3.2 at% ' C Sn = = CSn APb C SnAPb + CPb ASn x 100 94.5 (207.2 g / mol) x 100 94.5(207.2 g / mol) + 5.5(118.69 g / mol) = 96.8 at% 4.13 This problem calls for a conversion of composition in atom percent to composition in weight percent. The composition in atom percent for Problem 4.11 is 44.8 at% Ag, 46.2 at% Au, and 9.0 at% Cu. Modification of Equation (4.7) to take into account a three-component alloy leads to the following C Ag = ' C AgA Ag C' A Ag Ag = + C' A Au Au + C' A x 100 Cu Cu (44.8)(107.87 g / mol) x 100 (44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol) = 33.3 wt% C Au = = ' C AuA Au ' ' ' CAg AAg + C AuA Au + CCu ACu x 100 (46.2)(196.97 g / mol) x 100 (44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol) 69
- 72. = 62.7 wt% CCu = = ' C CuA Cu ' ' C 'AgAAg + C AuA Au + CCu ACu x 100 (9.0)(63.55 g / mol) x 100 (44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol) = 4.0 wt% 4.14 This problem calls for a determination of the number of atoms per cubic meter for aluminum. In order to solve this problem, one must employ Equation (4.2), N = NA ρ Al A Al 3 The density of Al (from the table inside of the front cover) is 2.71 g/cm , while its atomic weight is 26.98 g/mol. Thus, N = (6.023 23 x 10 )( atoms/ mol 2.71 g / cm 3 ) 26.98 g / mol = 6.05 x 1022 atoms/cm3 = 6.05 x 1028 atoms/m3 4.15 In order to compute the concentration in kg/m3 of Si in a 0.25 wt% Si-99.75 wt% Fe alloy we must employ Equation (4.9) as '' CSi = CSi CSi ρSi + CFe x 103 ρFe From inside the front cover, densities for silicon and iron are 2.33 and 7.87 g/cm3, respectively; and, therefore '' CSi = 0.25 0.25 2.33 g / cm3 + 70 99.75 7.87 g / cm3 x 103
- 73. = 19.6 kg/m3 4.16 We are asked in this problem to determine the approximate density of a high-leaded brass that has a composition of 64.5 wt% Cu, 33.5 wt% Zn, and 2 wt% Pb. In order to solve this problem, Equation (4.10a) is modified to take the following form: ρ ave = C Cu ρ Cu 100 C Zn + ρZn + CPb ρPb And, using the density values for Cu, Zn, and Pb that appear inside the front cover of the text, the density is computed as follows: ρ ave = 64.5 wt% 8.94 g / cm3 + 100 33.5 wt% 7.13 g / cm 3 + 2 wt% 11.35 g / cm3 = 8.27 g/cm3 4.17 This problem asks that we derive Equation (4.17), using other equations given in the chapter. The ' ' ' concentration of component 1 in atom percent (C1) is just 100 c 1 where c 1 is the atom fraction of ' ' component 1. Furthermore, c 1 is defined as c 1 = N1/N where N1 and N are, respectively, the number of atoms of component 1 and total number of atoms per cubic centimeter. Thus, from the above the following holds: N1 = ' C1 N 100 Substitution into this expression of the appropriate form of N from Equation (4.2) yields N1 = ' C1 N A ρave 100 A ave 71
- 74. ' Finally, substitution into this equation expressions for C1 [Equation (4.6a)], ρave [Equation (4.10a)], Aave [Equation (4.11a)], realizing that C2 = (C1 - 100), and after some algebraic manipulation we obtain the desired expression: NA C1 N1 = C1 A 1 ρ + 1 A1 ρ (100 − 2 C1 ) 4.18 This problem asks us to determine the number of molybdenum atoms per cubic centimeter for a 16.4 wt% Mo-83.6 wt% W solid solution. To solve this problem, employment of Equation (4.17) is necessary, using the following values: C1 = CMo = 16.4 wt% ρ1 = ρMo = 10.22 g/cm3 ρ2 = ρW = 19.3 g/cm3 A1 = AMo = 95.94 g/mol Thus NMo = NA CMo CMo A Mo A Mo + ρ ρ Mo = (6.023 W 100 ( − CMo ) ) x 10 23 atoms / mol (16.4) (16.4)(95.94 g / mol) (10.22 g / cm 3 ) + 95.94 g / mol 19.3 g / cm 3 (100 − 16.4 ) = 1.73 x 1022 atoms/cm3 4.19 This problem asks us to determine the number of niobium atoms per cubic centimeter for a 24 wt% Nb-76 wt% V solid solution. To solve this problem, employment of Equation (4.17) is necessary, using the following values: C1 = CNb = 24 wt% ρ1 = ρNb = 8.57 g/cm3 ρ2 = ρV = 6.10 g/cm3 72
- 75. A1 = ANb = 92.91 g/mol Thus NNb = = NACNb CNb ANb ANb + 100 − CNb ρNb ρV ( (6.023 x 1023 (24)(92.91 g / mol) (8.57 g / cm 3 ) ) atoms / mol (24) 92.91 g / mol + ) 6.10 g / cm3 (100 − 24) = 1.02 x 1022 atoms/cm3 4.20 This problem asks that we derive Equation (4.18), using other equations given in the chapter. The number of atoms of component 1 per cubic centimeter is just equal to the atom fraction of ' component 1 (c 1) times the total number of atoms per cubic centimeter in the alloy (N). Thus, using the equivalent of Equation (4.2), we may write ' c1 NA ρave ' N1 = c1 N = A ave Realizing that ' c1 = ' C1 100 and ' C '2 = 100 − C1 and substitution of the expressions for ρave and Aave, Equations (4.10b) and (4.11b) leads to N1 = ' c1 N Aρ ave Aave 73
- 76. = N C' ρ ρ A 1 1 2 ⎛ ' '⎞ A C1 ρ2 A1 + ⎜100 − C1 ⎟ ρ1 2 ⎠ ⎝ ' And, solving for C1 ' C1 = 100 N ρ A 1 1 2 NAρ1 ρ2 − N1ρ 2 A 1 + N1 ρ1 A 2 ' Substitution of this expression for C1 into Equation (4.7a) C1 = C' A 1 1 ' 1 1 + C 2A 2 C' A C' A 1 1 = ⎛ ⎞ ' 1 1 + 100⎜ 1 − C1⎟ A 2 ⎝ ⎠ C' A yields C1 = 1+ 100 NA ρ 2 N1 A1 − ρ2 ρ1 the desired expression. 4.21 This problem asks us to determine the weight percent of Au that must be added to Ag such that the resultant alloy will contain 5.5 x 1021 Au atoms per cubic centimeter. To solve this problem, employment of Equation (4.18) is necessary, using the following values: N1 = NAu = 5.5 x 1021 atoms/cm3 ρ1 = ρAu = 19.32 g/cm3 ρ2 = ρAg = 10.49 g/cm3 A1 = AAu = 196.97 g/mol A2 = Ag = 107.87 g/mol 74
- 77. Thus C Au = 1+ 100 NAρ Ag N A − Au Au = 1+ (6.023 ρ Ag ρ Au 100 ) x 10 23 atoms / mol (10.49 g / cm3 ) (5.5 x 10 21 atoms / cm3 )(196.97 g / mol) ⎛ 10.49 g / cm 3 ⎞ − ⎜ ⎟ ⎜ 3⎟ ⎝ 19.32 g / cm ⎠ = 15.9 wt% 4.22 This problem asks us to determine the weight percent of Ge that must be added to Si such that the resultant alloy will contain 2.43 x1021 Ge atoms per cubic centimeter. To solve this problem, employment of Equation (4.18) is necessary, using the following values: N1 = NGe = 2.43 x 1021 atoms/cm3 ρ1 = ρGe = 5.32 g/cm3 ρ2 = ρSi = 2.33 g/cm3 A1 = AGe = 72.59 g/mol A2 = ASi = 28.09 g/mol Thus C Ge = 1+ 100 N Aρ Si N GeA Ge − ρSi ρ Ge 100 = (6.023 x10 atoms/ mol)(2.33 g / cm 3 ) − ⎛⎜ 2.33 g/ cm 3 ⎞⎟ (2.43 x10 21 atoms / cm3 )(72.59 g / mol) ⎜⎝ 5.32 g/ cm 3 ⎟⎠ 23 1+ = 11.7 wt% 4.23 This problems asks that we compute the unit cell edge length for a 95 wt% Pt-5 wt% Cu alloy. First of all, the atomic radii for Cu and Pt (Table 3.1) are 0.1278 and 0.1387 nm, respectively. Also, using 75
- 78. Equation (3.5) it is possible to compute the unit cell volume, and inasmuch as the unit cell is cubic, the unit cell edge length is just the cube root of the volume. However, it is first necessary to calculate the density and atomic weight of this alloy using Equations (4.10a) and (4.11a). For the density ρ ave = 100 C Cu ρ Cu = CPt + ρPt 100 5 wt% 8.94 g / cm3 + 95 wt% 21.45 g / cm 3 = 20.05 g/cm3 And for the atomic weight Aave = 100 C Cu A Cu = + CPt APt 100 5 wt% 95 wt% + 63.55 g / mole 195.08 g / mol = 176.79 g/mol Now, VC is determined from Equation (3.5) as VC = = nA ave ρave NA (4 atoms / unitcell)(176.79 g / mol) (20.05 g / cm 3 )(6.023 x1023 = 5.856 x 10-23 cm3/unit cell And, finally 76 ) atoms / mol
- 79. ( ) a = VC ( = 5.856x10 − 23 1/ 3 3 cm /unit cell ) 1/3 = 3.883 x 10-8 cm = 0.3883 nm 4.24 The Burgers vector and dislocation line are perpendicular for edge dislocations, parallel for screw dislocations, and neither perpendicular nor parallel for mixed dislocations. 4.25 (a) The Burgers vector will point in that direction having the highest linear density. From Section 3.11, the linear density for the [110] direction in FCC is 1/2R, the maximum possible; therefore for FCC b = a [110] 2 From Problem 3.46 the linear density for the [111] direction in BCC is also 1/2R, and therefore for BCC b = a [111] 2 For simple cubic, a unit cell of which is shown in Figure 3.19, the atom spheres touch one another along the cube edges (i.e., in [100] directions) and therefore, the atomic packing is greatest in these directions. Therefore, the Burgers vector is b = a [100] 2 (b) For Cu which has an FCC crystal structure, R = 0.1278 nm (Table 3.1) and a = 2R 2 = 0.3615 nm [Equation (3.1)]; therefore b = = 0.3615 nm 2 a 2 h 2 + k 2 + l2 (1 )2 + (1 )2 + (0) 2 = 0.2556 nm 77
- 80. For Fe which has a BCC crystal structure, R = 0.1241 nm (Table 3.1) and a = 4R = 0.2866 3 nm [Equation (3.3)]; hence b = 0.2866 nm 2 (1) 2 + (1) 2 + (1) 2 = 0.2482 nm 4.26 (a) The surface energy of a single crystal depends on crystallographic orientation because the atomic packing is different for the various crystallographic planes, and, therefore, the number of unsatisfied bonds will vary from plane to plane. (b) The surface energy will be greater for an FCC (100) plane than for a (111) plane because the (111) plane is more densely packed (i.e., has more nearest neighbor atoms in the plane)—see Problem 3.47; as a consequence, more atomic bonds will be satisfied for the (111) plane, giving rise to a lower surface energy. 4.27 (a) The surface energy will be greater than the grain boundary energy since some atoms on one side of the boundary will bond to atoms on the other side--i.e., there will be fewer unsatisfied bonds along a grain boundary. (b) The small angle grain boundary energy is lower than for a high angle one because more atoms bond across the boundary for the small angle, and, thus, there are fewer unsatisfied bonds. 4.28 (a) A twin boundary is an interface such that atoms on one side are located at mirror image positions of those atoms situated on the other boundary side. The region on one side of this boundary is called a twin. (b) Mechanical twins are produced as a result of mechanical deformation and generally occur in BCC and HCP metals. Annealing twins form during annealing heat treatments, most often in FCC metals. 4.29 (a) The interfacial defect that exists for this stacking sequence is a twin boundary, which occurs at the following position 78
- 81. The stacking sequence on one side of this position is mirrored on the other side. (b) The interfacial defect that exists within this FCC stacking sequence is a stacking fault, which occurs over the region indicated For this region, the BCBC stacking sequence is HCP. 4.30 (a) This problem calls for a determination of the average grain size of the specimen which microstructure is shown in Figure 4.12b. Seven line segments were drawn across the micrograph, each of which was 60 mm long. The average number of grain boundary intersections for these lines was 8.7. Therefore, the average line length intersected is just 60 mm = 6.9 mm 8.7 Hence, the average grain diameter, d, is d = ave. line length int er sec ted 6.9 mm = = 6.9 x 10 −2 mm magnification 100 (b) This portion of the problem calls for us to estimate the ASTM grain size number for this same material. The average grain size number, n, is related to the number of grains per square inch, N, at a magnification of 100x according to Equation 4.16. Inasmuch as the magnification is 100x, the value of N is measured directly from the micrgraph, which is approximately 12 grains. Rearranging Equation 4.16 and solving for n leads to n= = log N +1 log 2 log 12 + 1 = 4.6 log 2 4.31 (a) This portion of the problem calls for a determination of the average grain size of the specimen which microstructure is shown in Figure 9.22a. 79 Seven line segments were drawn across the
- 82. micrograph, each of which was 60 mm long. The average number of grain boundary intersections for these lines was 6.3. Therefore, the average line length intersected is just 60 mm = 9.5 mm 6.3 Hence, the average grain diameter, d, is d = ave. line length int er sec ted 9.5 mm = = 0.106 mm magnification 90 (b) This portion of the problem calls for us to estimate the ASTM grain size number for this same material. The average grain size number, n, is related to the number of grains per square inch, N, at a magnification of 100x according to Equation 4.16. However, the magnification of this micrograph is not 100x, but rather 90x. Consequently, it is necessary to use the following equation: 2 ⎛ M ⎞ n−1 NM ⎜ ⎟ =2 ⎝ 100 ⎠ where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size number. (The above equation makes use of the fact that, while magnification is a length parameter, area is expressed in terms of units of length squared. As a consequence, the number of grains per unit area increases with the square of the increase in magnification.) Solving the above expression for n leads to ⎛ M ⎞ log NM + 2 log ⎜ ⎟ ⎝ 100⎠ n= +1 log 2 From Figure 9.22a, NM is measured to be approximately 4, which leads to ⎛ 90 ⎞ ⎟ log 4 + 2 log ⎜ ⎝ 100 ⎠ n= +1 log 2 = 2.7 80
- 83. 4.32 (a) This part of problem asks that we compute the number of grains per square inch for an ASTM grain size of 6 at a magnification of 100x. All we need do is solve for the parameter N in Equation 4.16, inasmuch as n = 6. Thus N = 2 n− 1 =2 6 −1 = 32 grains/in.2 (b) Now it is necessary to compute the value of N for no magnification. In order to solve this problem it is necessary to use the following equation: 2 ⎛ M ⎞ n−1 NM ⎜ ⎟ =2 ⎝ 100 ⎠ where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size number. (The above equation makes use of the fact that, while magnification is a length parameter, area is expressed in terms of units of length squared. As a consequence, the number of grains per unit area increases with the square of the increase in magnification.) Without any magnification, M in the above equation is 1, and therefore, 2 ⎛ 1 ⎞ 6 −1 N1 ⎜ ⎟ =2 = 32 ⎝ 100⎠ And, solving for N1, N1 = 320,000 grains/in.2. 4.33 This problem asks that we determine the ASTM grain size number if 30 grains per square inch are measured at a magnification of 250. In order to solve this problem we make use of the equation cited in Problem 4.31b—i.e., 2 ⎛ M ⎞ n−1 NM ⎜ ⎟ =2 ⎝ 100 ⎠ where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size number. Solving the above equation for n, and realizing that NM = 30, while M = 250, we have 81
- 84. ⎛ M ⎞ log NM + 2 log ⎜ ⎟ ⎝ 100⎠ n= +1 log 2 ⎛ 250 ⎞ ⎟ log 30 + 2 log ⎜ ⎝ 100 ⎠ = + 1 = 2.5 log 2 4.34 This problem asks that we determine the ASTM grain size number if 25 grains per square inch are measured at a magnification of 75. In order to solve this problem we make use of the equation cited in Problem 4.31b—i.e., 2 ⎛ M ⎞ n−1 NM ⎜ ⎟ =2 ⎝ 100 ⎠ where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size number. Solving the above equation for n, and realizing that NM = 25, while M = 75, we have ⎛ M ⎞ log NM + 2 log ⎜ ⎟ ⎝ 100⎠ n= +1 log 2 ⎛ 75 ⎞ log 25 + 2 log ⎜ ⎟ ⎝ 100 ⎠ = + 1 = 4.8 log 2 Design Problems 4.D1 This problem calls for us to compute the concentration of lithium (in wt%) that, when added to aluminum, will yield an alloy having a density of 2.55 g/cm3. Solution of this problem requires the use of Equation (4.10a), which takes the form ρ ave = CLi ρ Li + 100 100 − CLi ρ Al inasmuch as CLi + CAl = 100. According to the table inside the front cover, the respective densities of Li and Al are 0.534 and 2.71 g/cm3. Upon solving for C from the above equation Li 82
- 85. ( ρave ( Al − ρ 100 ρ Li ρAl − ρ ave CLi = ( (100) 0.534 g / cm = ( 3 ρLi ) )(2.71 g / cm3 − ) 2.55 g / cm 2.55 g/ cm3 2.71 g / cm3 − 0.534 g / cm3 ) 3 ) = 1.537 wt% 4.D2 This problem asks that we determine the concentration (in weight percent) of V that must be added to Fe so as to yield a unit cell edge length of 0.289 nm. To begin, it is necessary to employ Equation (3.5), and solve for the unit cell volume, VC, as nA ave VC = ρave NA where Aave and ρave are the atomic weight and density, respectively, of the Fe-V alloy. Inasmuch as both of these materials have the BCC crystal structure, which has cubic symmetry, VC is just the cube of the unit cell length, a. That is VC = a3 = (0.289 nm)3 (2.89 x 10 −8 cm) = 2.414 x 10−23 cm 3 3 It is now necessary to construct expressions for Aave and ρave in terms of the concentration of vanadium, CV using Equations (4.11a) and (4.10a). For Aave we have Aave = = 100 CV (100 − C V ) + AV AFe 100 CV 50.94 g / mol + whereas for ρave 83 (100 − CV ) 55.85 g / mol
- 86. ρ ave = = 100 (100 − C V ) + ρV ρFe CV 100 CV 6.10 g / cm 3 + (100 − C V ) 7.87 g / cm 3 Within the BCC unit cell there are 2 equivalent atoms, and thus, the value of n in Equation (3.5) is 2; hence, this expression may be written in terms of the concentration of V in weight percent as follows: VC = 2.414 x 10-23 cm3 = nAave ρaveN A ⎡ ⎤ ⎢ ⎥ 100 ⎥ (2 atoms / unit cell) ⎢ (100 − CV ) ⎥ CV ⎢ + ⎢ ⎥ 55.85 g/ mol ⎦ ⎣ 50.94 g / mol = ⎡ ⎤ ⎢ ⎥ 100 23 ⎢ ⎥ atoms / mol 6.023 x 10 ⎢ CV (100 − C V ) ⎥ + ⎢ ⎥ 3 7.87 g / cm3 ⎦ ⎢ ⎥ ⎣ 6.10 g / cm ( And solving this expression for CV leads to CV = 12.9 wt%. 84 )
- 87. CHAPTER 5 DIFFUSION PROBLEM SOLUTIONS 5.1 Self-diffusion is atomic migration in pure metals--i.e., when all atoms exchanging positions are of the same type. Interdiffusion is diffusion of atoms of one metal into another metal. 5.2 Self-diffusion may be monitored by using radioactive isotopes of the metal being studied. The motion of these isotopic atoms may be monitored by measurement of radioactivity level. 5.3 (a) With vacancy diffusion, atomic motion is from one lattice site to an adjacent vacancy. Selfdiffusion and the diffusion of substitutional impurities proceed via this mechanism. On the other hand, atomic motion is from interstitial site to adjacent interstitial site for the interstitial diffusion mechanism. (b) Interstitial diffusion is normally more rapid than vacancy diffusion because: (1) interstitial atoms, being smaller, are more mobile; and (2) the probability of an empty adjacent interstitial site is greater than for a vacancy adjacent to a host (or substitutional impurity) atom. 5.4 Steady-state diffusion is the situation wherein the rate of diffusion into a given system is just equal to the rate of diffusion out, such that there is no net accumulation or depletion of diffusing species--i.e., the diffusion flux is independent of time. 5.5 (a) The driving force is that which compels a reaction to occur. (b) The driving force for steady-state diffusion is the concentration gradient. 5.6 This problem calls for the mass of hydrogen, per hour, that diffuses through a Pd sheet. It first becomes necessary to employ both Equations (5.1a) and (5.3). Combining these expressions and solving for the mass yields M = JAt = − DAt ∆C ∆x ⎡ 0.6 − 2.4 kg / m 3 ⎤ ⎥ = − 1.0 x 10-8 m2 /s 0.2 m2 (3600 s/h) ⎢ −3 m ⎥ ⎢ ⎣ 5 x 10 ⎦ ( )( ) 85
- 88. = 2.6 x 10-3 kg/h 3 5.7 We are asked to determine the position at which the nitrogen concentration is 2 kg/m . This problem is solved by using Equation (5.3) in the form C − C B J = − D A x − x A B 3 If we take C to be the point at which the concentration of nitrogen is 4 kg/m , then it becomes A necessary to solve for x , as B ⎡ C − CB ⎤ xB = x A + D ⎢ A ⎥ J ⎣ ⎦ Assume x is zero at the surface, in which case A ( -11 xB = 0 + 6 x 10 )( ⎡ 4 kg / m3 − 2 kg / m3 ⎢ m /s ⎢ −7 kg / m2 - s ⎢ 1.2 x 10 ⎣ 2 )⎤⎥ ⎥ ⎥ ⎦ = 1 x 10-3 m = 1 mm 5.8 This problem calls for computation of the diffusion coefficient for a steady-state diffusion situation. Let us first convert the carbon concentrations from wt% to kg C/m3 using Equation (4.9a). For 0.012 wt% C '' CC = CC CC ρC = 3 CFe + x 10 ρ Fe 0.012 0.012 2.25 g / cm3 + 99.988 7.87 g / cm3 0.944 kg C/m3 86 x 10 3
- 89. Similarly, for 0.0075 wt% C 0.0075 '' CC = 0.0075 2.25 g / cm3 + 99.9925 x 103 7.87 g/ cm3 = 0.590 kg C/m3 Now, using a form of Equation (5.3) ⎡ x − xB ⎤ D = − J ⎢ A ⎥ ⎢C A − CB ⎦ ⎥ ⎣ −3 ⎡ ⎤ − 10 m = − 1.40 x 10-8 kg/m2 - s ⎢ ⎥ 3 − 0.590 kg / m3 ⎥ ⎢0.944 kg / m ⎣ ⎦ ( ) = 3.95 x 10-11 m2/s 5.9 This problems asks for us to compute the diffusion flux of hydrogen gas through a 1-mm thick plate of iron at 250°C when the pressures on the two sides are 0.15 and 7.5 MPa. Ultimately we will employ Equation (5.3) to solve this problem. However, it first becomes necessary to determine the concentration of hydrogen at each face using Equation (5.11). At the low pressure (or B) side ( CH(B) = 1.34 x 10-2 27, 200 J / ) 0.15 MPa exp ⎢⎣⎡− (8.31 J / mol- K)(250mol 273 K)⎤⎥⎦ + 9.93 x 10-6 wt% Whereas, for the high pressure (or A) side ( CH(A) = 1.34 x 10-2 ) 7.5 27,200 J/ mol ⎤ ⎡ MPa exp ⎢− ⎦ ⎣ (8.31 J/ mol- K)(250 + 273 K) ⎥ 7.02 x 10-5 wt% 87
- 90. We now convert concentrations in weight percent to mass of hydrogen per unit volume of solid. At face B there are 9.93 x 10-6 g (or 9.93 x 10-9 kg) of hydrogen in 100 g of Fe, which is virtually pure iron. From the density of iron (7.87 g/cm3), the volume iron in 100 g (VB) is just VB = 100 g 7.87 g / cm 3 = 12.7 cm3 = 1.27 x 10-5 m3 Therefore, the concentration of hydrogen at the B face in kilograms of H per cubic meter of alloy '' [ CH(B) ] is just C H(B) '' CH(B) = = 9.93 x 10−9 kg 1.27 x 10−5 m3 V B -4 = 7.82 x 10 kg/m 3 At the A face the volume of iron in 100 g (VA) will also be 1.27 x 10-5 m3, and '' CH(A) = = 7.02 x 10−8 kg 1.27 x 10−5 m3 C H(A ) V A -3 = 5.53 x 10 3 kg/m Thus, the concentration gradient is just the difference between these concentrations of hydrogen divided by the thickness of the iron membrane; that is − C '' C '' ∆C H(B) H(A) = ∆x x − x B = A 7.82 x 10 −4 kg / m3 − 5.53 x 10−3 kg / m 3 10 −3 m = − 4.75 kg/m4 At this time it becomes necessary to calculate the value of the diffusion coefficient at 250°C using Equation (5.8). Thus, 88
- 91. ⎛ Q ⎞ D = D o exp ⎜ − o ⎟ ⎝ RT ⎠ ( = 1.4 x 10 ) ⎛ ⎞ 13, 400 J / mol 2 m / s exp ⎜ − ⎟ (8.31 J / mol − K)(250 + 273 K) ⎠ ⎝ −7 = 6.41 x 10-9 m2/s And, finally, the diffusion flux is computed using Equation (5.3) by taking the negative product of this diffusion coefficient and the concentration gradient, as J =−D ( -9 = − 6.41 x 10 2 ∆C ∆x )( 4 m /s − 4.75 kg/m )= 3.05 x 10-8 kg/m2 - s 5.10 It can be shown that ⎛ x2 ⎞ exp − ⎜ ⎜ 4 Dt ⎟ ⎟ Dt ⎝ ⎠ B Cx = is a solution to ∂C ∂2C = D 2 ∂t ∂x simply by taking appropriate derivatives of the C expression. When this is carried out, x 2 ∂C ∂ C B = D = 2 1/ 2t3 / 2 ∂t 2D ∂x 5.11 ⎛ x2 ⎞ ⎜ ⎜ 2 Dt − 1⎟ exp ⎟ ⎝ ⎠ ⎛ x2 ⎞ ⎜− ⎜ 4Dt ⎟ ⎟ ⎝ ⎠ We are asked to compute the diffusion time required for a specific nonsteady-state diffusion situation. It is first necessary to use Equation (5.5). ⎛ x ⎞ = 1 − erf ⎜ ⎟ C −C ⎝ 2 Dt ⎠ s o C x − Co 89
- 92. -3 wherein, C = 0.45, C = 0.20, C = 1.30, and x = 2 mm = 2 x 10 m. Thus, x o s C x − Co C −C s o = ⎛ x ⎞ 0.45 − 0.20 ⎟ = 0.2273 = 1 − erf ⎜ 1.30 − 0.20 ⎝ 2 Dt ⎠ or ⎛ x ⎞ erf ⎜ ⎟ = 1 − 0.2273 = 0.7727 ⎝ 2 Dt ⎠ By linear interpolation from Table 5.1 z erf(z) 0.85 0.7707 z 0.7727 0.90 0.7970 z − 0.850 0.7727 − 0.7707 = 0.900 − 0.850 0.7970 − 0.7707 From which z = 0.854 = x 2 Dt Now, from Table 5.2, at 1000°C (1273 K) ( ) ⎤ ⎡ 148, 000 J / mol D = 2.3 x 10-5 m2 /s exp ⎢− ⎥ ⎣ (8.31 J / mol-K)(1273 K) ⎦ -11 2 = 1.93 x 10 m /s Thus, 0.854 = ( 2 x 10−3 m ) (2) 1.93x10−11 m2 / s (t) 90
- 93. Solving for t yields 4 t = 7.1 x 10 s = 19.7 h 5.12 This problem asks that we determine the position at which the carbon concentration is 0.25 wt% after a 10-h heat treatment at 1325 K when Co = 0.55 wt% C. From Equation (5.5) C x − Co C −C s o = ⎛ x ⎞ 0.25 − 0.55 = 0.5455 = 1 − erf ⎜ ⎟ 0 − 0.55 ⎝ 2 Dt ⎠ Thus, ⎛ x ⎞ erf ⎜ ⎟ = 0.4545 ⎝ 2 Dt ⎠ Using data in Table 5.1 and linear interpolation z erf (z) 0.40 0.4284 z 0.4545 0.45 0.4755 z − 0.40 0.4545 − 0.4284 = 0.45 − 0.40 0.4755 − 0.4284 And, z = 0.4277 Which means that x 2 Dt = 0.4277 And, finally x = 2(0.4277) Dt = (0.8554) (4.3 x 10−11 m2 / s)(3.6 x 104 s ) = 1.06 x 10-3 m = 1.06 mm 91
- 94. 5.13 This problem asks us to compute the nitrogen concentration (C ) at the 1 mm position after a 10 h x diffusion time, when diffusion is nonsteady- state. From Equation (5.5) C x − Co C −C s ⎛ x ⎞ = 1 − erf ⎜ ⎟ 0.1 − 0 ⎝ 2 Dt ⎠ Cx − 0 = o ⎡ ⎢ = 1 − erf ⎢ ⎢ (2) ⎣ ⎤ ⎥ ⎥ −11 2 2.5 x 10 m / s (10 h)(3600 s / h) ⎥ ⎦ −3 10 ( m ) = 1 - erf (0.527) Using data in Table 5.1 and linear interpolation z erf (z) 0.500 0.5205 0.527 y 0.550 0.5633 0.527 − 0.500 y − 0.5205 = 0.550 − 0.500 0.5633 − 0.5205 from which y = erf (0.527) = 0.5436 Thus, Cx − 0 0.1 − 0 = 1.0 − 0.5436 This expression gives C = 0.046 wt% N x 5.14 (a) The solution to Fick's second law for a diffusion couple composed of two semi-infinite solids of the same material is as follows: 92
- 95. ⎛ C1 + C 2 ⎞ ⎛ C1 − C2 ⎞ ⎛ x ⎞ Cx = ⎜ ⎟ ⎟ − ⎜ ⎟ erf ⎜ 2 2 ⎝ ⎠ ⎝ ⎠ ⎝ 2 Dt ⎠ for the boundary conditions C = C1 for x < 0, and t = 0 C = C2 for x > 0, and t = 0 (b) For this particular silver-gold diffusion couple for which C1 = 5 wt% Au and C2 = 2 wt% Au, we are asked to determine the diffusion time at 750°C that will give a composition of 2.5 wt% Au at the 50 µm position. Thus, the equation in part (a) takes the form ⎛ 50 x 10 −6 m ⎞ ⎛ 5 + 2⎞ ⎛ 5 − 2⎞ 2.5 = ⎜ ⎟ − ⎜ ⎟ erf ⎜ ⎟ ⎜ ⎟ ⎝ 2 ⎠ ⎝ 2 ⎠ 2 Dt ⎝ ⎠ It now becomes necessary to compute the diffusion coefficient at 750°C (1023 K) given that Do = 8.5 x 10-5 m2/s and Qd = 202,100 J/mol. From Equation (5.8) we have ⎛ Q ⎞ D = D oexp ⎜ − d ⎟ ⎝ RT ⎠ ( -5 = 8.5 x 10 ) ⎡ ⎤ 202,100 J / mol 2 m /s exp⎢− ⎥ ⎣ (8.31J / mol − K)(1023 K) ⎦ = 4.03 x 10-15 m2/s Substitution of this value into the above equation leads to ⎡ ⎢ 5 + 2⎞ 5 − 2⎞ ⎛ ⎛ 2.5 = ⎜ ⎟ − ⎜ ⎟ erf ⎢ ⎝ 2 ⎠ ⎝ 2 ⎠ ⎢2 ⎣ This expression reduces to the following form: 93 ⎤ ⎥ ⎥ −15 2 4.03 x 10 m / s (t) ⎥ ⎦ −6 ( 50 x 10 m )
- 96. ⎛ 393.8 s ⎞ 0.6667 = erf ⎜ ⎟ t ⎠ ⎝ Using data in Table 5.1 and linear interpolation z erf (z) 0.650 0.6420 y 0.6667 0.700 0.6778 y − 0.650 0.6667 − 0.6420 = 0.700 − 0.650 0.6778 − 0.6420 from which y = 0.6844 = 393.8 s t And, solving for t gives t = 3.31 x 105 s = 92 h 5.15 This problem calls for an estimate of the time necessary to achieve a carbon concentration of 0.45 wt% at a point 5 mm from the surface. From Equation (5.6b), x2 = constant Dt But since the temperature is constant, so also is D constant, and x2 = constant t or 2 x1 t1 = Thus, 94 x2 2 t2

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

/s and @ 700°C is 3.9 ×

10-13 cm2

/s respectively. Estimate the energy required to diffuse one mole of carbon atoms into

FCC Ni.